# Electronic Supplementary Material (ESI) for Inorganic Chemistry Frontiers.
# This journal is © the Partner Organisations 2021

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_compound1
_database_code_depnum_ccdc_archive 'CCDC 2042532'
loop_
_audit_author_name
_audit_author_address
'Hai Fu'
;CCUT china
China
;
_audit_update_record             
;
2020-11-05 deposited with the CCDC.	2021-01-07 downloaded from the CCDC.
;
_audit_creation_date             2020-11-04
_audit_creation_method           
;
Olex2 1.2
(compiled 2014.09.19 svn.r3010 for OlexSys, GUI svn.r4874)
;
_chemical_formula_moiety         'Mo7 O24, H4 O2 Pd0.5, 7(H2 O), O'
_chemical_formula_sum            'H18 Mo7 O34 Pd0.5'
_chemical_formula_weight         1286.85
_chemical_absolute_configuration unk
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_Cromer_Mann_a1
_atom_type_scat_Cromer_Mann_a2
_atom_type_scat_Cromer_Mann_a3
_atom_type_scat_Cromer_Mann_a4
_atom_type_scat_Cromer_Mann_b1
_atom_type_scat_Cromer_Mann_b2
_atom_type_scat_Cromer_Mann_b3
_atom_type_scat_Cromer_Mann_b4
_atom_type_scat_Cromer_Mann_c
_atom_type_scat_source
_atom_type_scat_dispersion_source
H 0.00000 0.00000 0.49300 0.32291 0.14019 0.04081 10.51090 26.12570 3.14236
57.79970 0.0030380000826
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Mo -1.68402 0.70339 3.70250 17.23560 12.88760 3.74290 0.27720 1.09580 11.00400
61.65840 4.38749980927
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
O 0.01158 0.00611 3.04850 2.28680 1.54630 0.86700 13.27710 5.70110 0.32390
32.90890 0.250800013542
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Pd -0.98845 1.01473 19.33190 15.50170 5.29537 0.60584 0.69866 7.98929 25.20520
76.89860 5.26593017578
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'

_space_group_crystal_system      orthorhombic
_space_group_IT_number           43
_space_group_name_H-M_alt        'F d d 2'
_space_group_name_Hall           'F 2 -2d'
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,-y,z
3 -x+1/4,y+1/4,z+1/4
4 x+1/4,-y+1/4,z+1/4
5 x,y+1/2,z+1/2
6 -x,-y+1/2,z+1/2
7 -x+1/4,y+3/4,z+3/4
8 x+1/4,-y+3/4,z+3/4
9 x+1/2,y,z+1/2
10 -x+1/2,-y,z+1/2
11 -x+3/4,y+1/4,z+3/4
12 x+3/4,-y+1/4,z+3/4
13 x+1/2,y+1/2,z
14 -x+1/2,-y+1/2,z
15 -x+3/4,y+3/4,z+1/4
16 x+3/4,-y+3/4,z+1/4

_symmetry_Int_Tables_number      43
_cell_length_a                   19.203(2)
_cell_length_b                   72.352(8)
_cell_length_c                   8.3479(9)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     11598(2)
_cell_formula_units_Z            16
_cell_measurement_reflns_used    9870
_cell_measurement_theta_max      28.351
_cell_measurement_theta_min      3.010
_exptl_absorpt_coefficient_mu    3.351
_exptl_absorpt_correction_type   none
_exptl_crystal_density_diffrn    2.9478
_exptl_crystal_F_000             9516.9582
_diffrn_reflns_av_R_equivalents  0.0756
_diffrn_reflns_av_unetI/netI     0.0463
_diffrn_reflns_limit_h_max       25
_diffrn_reflns_limit_h_min       -25
_diffrn_reflns_limit_k_max       96
_diffrn_reflns_limit_k_min       -96
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            41964
_diffrn_reflns_theta_full        24.9997
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         2.68
_diffrn_measured_fraction_theta_full 0.9992
_diffrn_measured_fraction_theta_max 0.9992
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_reflns_Friedel_coverage         1.000
_reflns_limit_h_max              22
_reflns_limit_h_min              -22
_reflns_limit_k_max              85
_reflns_limit_k_min              -85
_reflns_limit_l_max              9
_reflns_limit_l_min              -9
_reflns_number_gt                4950
_reflns_number_total             5103
_reflns_threshold_expression     I>=2u(I)
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'olex2.refine (Bourhis et al., 2013)'
_refine_diff_density_max         0.9658
_refine_diff_density_min         -2.2416
_refine_diff_density_rms         0.1868
_refine_ls_abs_structure_details 
'Flack, H. D. (1983). Acta Cryst. A39, 876-881.'
_refine_ls_abs_structure_Flack   0.03(6)
_refine_ls_d_res_high            0.8409
_refine_ls_d_res_low             7.6133
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_goodness_of_fit_ref   1.0575
_refine_ls_hydrogen_treatment    refall
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     397
_refine_ls_number_reflns         5103
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0355
_refine_ls_R_factor_gt           0.0337
_refine_ls_restrained_S_all      1.0575
_refine_ls_shift/su_max          0.0971
_refine_ls_shift/su_mean         0.0010
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0430P)²+418.9836P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0858
_refine_ls_wR_factor_ref         0.0871
_olex2_refinement_description    
;
;
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Mo1 Mo -0.7382991(5) -0.3035024(5) -1.7609308(5) 0.01274(11) Uani 1.000000 1 .
. .
Mo2 Mo -0.8721615(5) -0.3482616(5) -1.6450625(5) 0.02123(12) Uani 1.000000 1 .
. .
Mo3 Mo -0.8728469(5) -0.2755427(5) -1.7665670(5) 0.01412(11) Uani 1.000000 1 .
. .
Mo4 Mo -1.0041949(5) -0.3202431(5) -1.6540153(5) 0.01688(12) Uani 1.000000 1 .
. .
Mo5 Mo -0.8832357(5) -0.3176194(5) -1.9536613(5) 0.01179(11) Uani 1.000000 1 .
. .
Mo6 Mo -0.7425025(5) -0.3453800(5) -1.8860457(5) 0.01664(12) Uani 1.000000 1 .
. .
Mo7 Mo -1.0216696(5) -0.2873494(5) -1.9068509(5) 0.01574(12) Uani 1.000000 1 .
. .
Pd1 Pd -0.75 -0.25 -2.3085067(4) 0.03223(19) Uani 1.000000 2 S T P
O1 O -0.8100936(5) -0.3268966(5) -1.7611918(5) 0.0122(6) Uani 1.000000 1 . . .
O2 O -0.7037093(5) -0.3211605(5) -1.9212370(5) 0.0190(6) Uani 1.000000 1 . . .
O3 O -0.8227100(5) -0.2972691(5) -1.9346615(5) 0.0142(6) Uani 1.000000 1 . . .
O4 O -0.9371812(5) -0.3347546(5) -1.8325624(5) 0.0138(6) Uani 1.000000 1 . . .
O5 O -0.9387870(5) -0.2993959(5) -1.7703761(5) 0.0140(6) Uani 1.000000 1 . . .
O6 O -0.6961302(5) -0.3116279(5) -1.5934220(5) 0.0219(6) Uani 1.000000 1 . . .
O7 O -0.9423481(5) -0.2715921(5) -1.9402298(5) 0.0194(6) Uani 1.000000 1 . . .
O8 O -1.0318204(5) -0.3047587(5) -1.5139275(5) 0.0322(7) Uani 1.000000 1 . . .
O9 O -0.9458320(5) -0.3085697(5) -2.0834240(5) 0.0220(7) Uani 1.000000 1 . . .
O10 O -0.8068356(5) -0.2891467(5) -1.6410900(5) 0.0166(6) Uani 1.000000 1 . . .
O11 O -0.6868379(5) -0.2859488(5) -1.8298934(5) 0.0210(6) Uani 1.000000 1 . . .
O12 O -0.6828230(5) -0.3530258(5) -1.7483557(5) 0.0248(6) Uani 1.000000 1 . . .
O13 O -1.0561165(5) -0.3109272(5) -1.8396808(5) 0.0175(6) Uani 1.000000 1 . . .
O14 O -1.0684007(5) -0.2736515(5) -1.7781941(5) 0.0279(7) Uani 1.000000 1 . . .
O15 O -0.9132460(5) -0.2644603(5) -1.6134649(5) 0.0259(7) Uani 1.000000 1 . . .
O16 O -0.9228577(5) -0.3285026(5) -1.5389500(5) 0.0204(6) Uani 1.000000 1 . . .
O17 O -0.8348997(5) -0.3325075(5) -2.0723151(5) 0.0202(6) Uani 1.000000 1 . . .
O18 O -0.8192793(5) -0.2592563(5) -1.8494167(5) 0.0275(6) Uani 1.000000 1 . . .
O19 O -0.9306492(5) -0.3657638(5) -1.6265160(5) 0.0362(6) Uani 1.000000 1 . . .
O20 O -0.7192679(5) -0.3561923(5) -2.0647150(5) 0.0277(7) Uani 1.000000 1 . . .
O24 O -1.0627726(5) -0.2850361(5) -2.0889321(5) 0.0278(7) Uani 1.000000 1 . . .
O21 O -0.8204077(5) -0.3600639(5) -1.8238100(5) 0.0255(6) Uani 1.000000 1 . . .
O23 O -1.0570572(5) -0.3389163(5) -1.6231276(5) 0.0294(6) Uani 1.000000 1 . . .
O22 O -0.8134224(5) -0.3517997(5) -1.4919681(5) 0.0390(7) Uani 1.000000 1 . . .
O1W O -0.7001172(5) -0.2645967(5) -2.4854740(5) 0.0527783(5) Uiso 1.000000 1 .
. .
H1Wa H -0.7258971(5) -0.2655659(5) -2.5678273(5) 0.0791674(5) Uiso 1.000000 1 .
. .
H1Wb H -0.6647051(5) -0.2586173(5) -2.5178824(5) 0.0791674(5) Uiso 1.000000 1 .
. .
O2W O -0.7102703(5) -0.2664612(5) -2.1344979(5) 0.0558906(5) Uiso 1.000000 1 .
. .
H2Wa H -0.6992006(5) -0.2596733(5) -2.0554269(5) 0.0838359(5) Uiso 1.000000 1 .
. .
H2Wb H -0.7418066(5) -0.2735594(5) -2.0981458(5) 0.0838359(5) Uiso 1.000000 1 .
. .
o3w O -0.6971103(5) -0.3064735(5) -2.2249268(5) 0.0365806(5) Uiso 1.000000 1 .
. .
H3wa H -0.6980498(5) -0.3176691(5) -2.2557838(5) 0.0548709(5) Uiso 1.000000 1 .
. .
H3wb H -0.6738519(5) -0.3000575(5) -2.2913924(5) 0.0548709(5) Uiso 1.000000 1 .
. .
o4w O -0.5656002(5) -0.3237688(5) -1.7253480(5) 0.0480371(5) Uiso 1.000000 1 .
. .
H4wa H -0.5738757(5) -0.3142173(5) -1.6692374(5) 0.0720557(5) Uiso 1.000000 1 .
. .
H4wb H -0.5486802(5) -0.3321949(5) -1.6660165(5) 0.0720557(5) Uiso 1.000000 1 .
. .
o5w O -0.6723754(5) -0.3450524(5) -1.3859898(5) 0.0490928(5) Uiso 1.000000 1 .
. .
H5wa H -0.6420342(5) -0.3365078(5) -1.3894856(5) 0.0736392(5) Uiso 1.000000 1 .
. .
H5wb H -0.6949682(5) -0.3439187(5) -1.4730232(5) 0.0736392(5) Uiso 1.000000 1 .
. .
o6w O -0.5352522(5) -0.3535780(5) -1.5152762(5) 0.0529796(5) Uiso 1.000000 1 .
. .
o7w O -1.0437796(5) -0.2683530(5) -1.4091373(5) 0.0576658(5) Uiso 1.000000 1 .
. .
o8w O -0.8327110(5) -0.3749702(5) -1.2174755(5) 0.0606300(5) Uiso 1.000000 1 .
. .
o9w O -0.8379098(5) -0.3046033(5) -1.3509954(5) 0.0573700(5) Uiso 1.000000 1 .
. .
o10w O -0.9038616(5) -0.2698099(5) -2.2502420(5) 0.0667575(5) Uiso 1.000000 1 .
. .
H10a H -0.8622793(5) -0.2676478(5) -2.2796937(5) 0.1001363(5) Uiso 1.000000 1 .
. .
H10b H -0.9292482(5) -0.2715676(5) -2.3322509(5) 0.1001363(5) Uiso 1.000000 1 .
. .
H6wa H -0.5587299(5) -0.3630926(5) -1.5407927(5) 0.0794693(5) Uiso 1.000000 1 .
. .
H6wb H -0.5440518(5) -0.3506595(5) -1.4187457(5) 0.0794693(5) Uiso 1.000000 1 .
. .
H7wa H -1.0421589(5) -0.2790703(5) -1.4506826(5) 0.0864986(5) Uiso 1.000000 1 .
. .
H7wb H -1.0473632(5) -0.2693181(5) -1.3079947(5) 0.0864986(5) Uiso 1.000000 1 .
. .
H9wa H -0.8282468(5) -0.2997963(5) -1.4412053(5) 0.0860549(5) Uiso 1.000000 1 .
. .
H9wb H -0.8662426(5) -0.3134975(5) -1.3643458(5) 0.0860549(5) Uiso 1.000000 1 .
. .


loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 Mo3 3.2817(3) . ?
Mo1 Mo5 3.3731(3) . ?
Mo1 Mo6 3.2059(3) . ?
Mo1 O1 2.18302(18) . ?
Mo1 O2 1.96577(14) . ?
Mo1 O3 2.22128(18) . ?
Mo1 O6 1.71950(13) . ?
Mo1 O10 1.95236(14) . ?
Mo1 O11 1.70907(13) . ?
Mo2 Mo4 3.2470(3) . ?
Mo2 Mo5 3.4054(3) . ?
Mo2 Mo6 3.2077(3) . ?
Mo2 O1 2.17942(15) . ?
Mo2 O4 2.22797(16) . ?
Mo2 O16 1.94323(14) . ?
Mo2 O19 1.69968(14) . ?
Mo2 O21 1.98580(14) . ?
Mo2 O22 1.72369(14) . ?
Mo3 Mo5 3.4274(3) . ?
Mo3 Mo7 3.2044(3) . ?
Mo3 O3 2.31668(16) . ?
Mo3 O5 2.14075(18) . ?
Mo3 O7 1.99112(16) . ?
Mo3 O10 1.91645(14) . ?
Mo3 O15 1.69654(12) . ?
Mo3 O18 1.71024(12) . ?
Mo4 Mo5 3.4188(3) . ?
Mo4 Mo7 3.1987(2) . ?
Mo4 O4 2.23157(15) . ?
Mo4 O5 2.19001(15) . ?
Mo4 O8 1.70415(12) . ?
Mo4 O13 1.96230(15) . ?
Mo4 O16 1.92854(17) . ?
Mo4 O23 1.70945(14) . ?
Mo5 Mo6 3.4141(3) . ?
Mo5 Mo7 3.4664(3) . ?
Mo5 O1 2.23713(17) . ?
Mo5 O3 1.88252(15) . ?
Mo5 O4 1.90579(13) . ?
Mo5 O5 2.28416(15) . ?
Mo5 O9 1.74556(13) . ?
Mo5 O17 1.73290(12) . ?
Mo6 O1 2.13526(15) . ?
Mo6 O2 1.92662(18) . ?
Mo6 O12 1.71479(13) . ?
Mo6 O17 2.53640(19) . ?
Mo6 O20 1.74231(14) . ?
Mo6 O21 1.90698(16) . ?
Mo7 O5 2.14259(17) . ?
Mo7 O7 1.92288(17) . ?
Mo7 O9 2.57889(17) . ?
Mo7 O13 1.91365(17) . ?
Mo7 O14 1.71493(11) . ?
Mo7 O24 1.72086(15) . ?
Pd1 O1W 2.05312(14) 14_345 ?
Pd1 O1W 2.05312(14) . ?
Pd1 O2W 2.02746(14) . ?
Pd1 O2W 2.02746(14) 14_345 ?
O1W H1Wa 0.85006(7) . ?
O1W H1Wb 0.85015(8) . ?
O2W H2Wa 0.84975(7) . ?
O2W H2Wb 0.85004(7) . ?
o3w H3wa 0.85018(9) . ?
o3w H3wb 0.85019(6) . ?
o4w H4wa 0.84984(8) . ?
o4w H4wb 0.85003(7) . ?
o5w H5wa 0.85000(8) . ?
o5w H5wb 0.85018(7) . ?
o6w H6wa 0.85001(8) . ?
o6w H6wb 0.85000(8) . ?
o7w H7wa 0.85001(9) . ?
o7w H7wb 0.85000(9) . ?
o9w H9wa 0.85000(8) . ?
o9w H9wb 0.85002(8) . ?
o10w H10a 0.85000(10) . ?
o10w H10b 0.85000(7) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Mo5 Mo1 Mo3 61.9802(7) . . ?
Mo6 Mo1 Mo3 123.9240(7) . . ?
Mo6 Mo1 Mo5 62.4610(7) . . ?
O1 Mo1 Mo3 88.8963(8) . . ?
O1 Mo1 Mo5 40.8579(7) . . ?
O1 Mo1 Mo6 41.4948(8) . . ?
O2 Mo1 Mo3 131.0625(5) . . ?
O2 Mo1 Mo5 75.9533(7) . . ?
O2 Mo1 Mo6 34.1551(10) . . ?
O2 Mo1 O1 73.0696(13) . . ?
O3 Mo1 Mo3 44.8454(8) . . ?
O3 Mo1 Mo5 31.5658(10) . . ?
O3 Mo1 Mo6 87.7538(11) . . ?
O3 Mo1 O1 72.2979(10) . . ?
O3 Mo1 O2 86.2185(8) . . ?
O6 Mo1 Mo3 126.3817(9) . . ?
O6 Mo1 Mo5 132.2932(16) . . ?
O6 Mo1 Mo6 87.3444(17) . . ?
O6 Mo1 O1 91.8981(16) . . ?
O6 Mo1 O2 99.9208(17) . . ?
O6 Mo1 O3 160.7378(11) . . ?
O10 Mo1 Mo3 31.6469(5) . . ?
O10 Mo1 Mo5 81.3327(7) . . ?
O10 Mo1 Mo6 130.7505(13) . . ?
O10 Mo1 O1 89.2717(11) . . ?
O10 Mo1 O2 157.2736(9) . . ?
O10 Mo1 O3 74.6119(8) . . ?
O10 Mo1 O6 94.7396(8) . . ?
O11 Mo1 Mo3 89.5593(15) . . ?
O11 Mo1 Mo5 122.7809(8) . . ?
O11 Mo1 Mo6 127.3830(10) . . ?
O11 Mo1 O1 160.2184(5) . . ?
O11 Mo1 O2 93.3415(11) . . ?
O11 Mo1 O3 92.9302(12) . . ?
O11 Mo1 O6 104.8158(11) . . ?
O11 Mo1 O10 99.615(2) . . ?
Mo5 Mo2 Mo4 61.7955(6) . . ?
Mo6 Mo2 Mo4 123.4395(10) . . ?
Mo6 Mo2 Mo5 62.0780(6) . . ?
O1 Mo2 Mo4 88.5080(12) . . ?
O1 Mo2 Mo5 40.1730(5) . . ?
O1 Mo2 Mo6 41.4496(9) . . ?
O4 Mo2 Mo4 43.3151(6) . . ?
O4 Mo2 Mo5 31.5689(7) . . ?
O4 Mo2 Mo6 88.0442(5) . . ?
O4 Mo2 O1 71.5098(10) . . ?
O16 Mo2 Mo4 32.8617(4) . . ?
O16 Mo2 Mo5 80.4801(12) . . ?
O16 Mo2 Mo6 128.8228(16) . . ?
O16 Mo2 O1 87.4171(17) . . ?
O16 Mo2 O4 73.5495(11) . . ?
O19 Mo2 Mo4 87.2073(11) . . ?
O19 Mo2 Mo5 120.8425(6) . . ?
O19 Mo2 Mo6 128.2023(14) . . ?
O19 Mo2 O1 158.4836(4) . . ?
O19 Mo2 O4 91.1740(10) . . ?
O19 Mo2 O16 100.1107(11) . . ?
O21 Mo2 Mo4 129.9368(7) . . ?
O21 Mo2 Mo5 75.0938(10) . . ?
O21 Mo2 Mo6 33.7212(10) . . ?
O21 Mo2 O1 72.3661(11) . . ?
O21 Mo2 O4 86.6275(7) . . ?
O21 Mo2 O16 155.4503(18) . . ?
O21 Mo2 O19 94.5177(17) . . ?
O22 Mo2 Mo4 128.3703(13) . . ?
O22 Mo2 Mo5 134.3017(15) . . ?
O22 Mo2 Mo6 88.0932(5) . . ?
O22 Mo2 O1 94.4322(12) . . ?
O22 Mo2 O4 162.315(2) . . ?
O22 Mo2 O16 95.6872(12) . . ?
O22 Mo2 O19 104.7271(17) . . ?
O22 Mo2 O21 99.5428(11) . . ?
Mo5 Mo3 Mo1 60.3191(7) . . ?
Mo7 Mo3 Mo1 122.8908(12) . . ?
Mo7 Mo3 Mo5 62.9199(7) . . ?
O3 Mo3 Mo1 42.5440(5) . . ?
O3 Mo3 Mo5 31.2925(7) . . ?
O3 Mo3 Mo7 88.1878(8) . . ?
O5 Mo3 Mo1 88.2196(13) . . ?
O5 Mo3 Mo5 40.7758(7) . . ?
O5 Mo3 Mo7 41.5955(8) . . ?
O5 Mo3 O3 71.9280(12) . . ?
O7 Mo3 Mo1 128.8017(11) . . ?
O7 Mo3 Mo5 75.9190(12) . . ?
O7 Mo3 Mo7 34.3508(9) . . ?
O7 Mo3 O3 86.2699(9) . . ?
O7 Mo3 O5 73.0495(11) . . ?
O10 Mo3 Mo1 32.3111(5) . . ?
O10 Mo3 Mo5 80.2920(14) . . ?
O10 Mo3 Mo7 130.7466(17) . . ?
O10 Mo3 O3 73.0040(11) . . ?
O10 Mo3 O5 89.1572(16) . . ?
O10 Mo3 O7 156.208(2) . . ?
O15 Mo3 Mo1 129.8318(7) . . ?
O15 Mo3 Mo5 137.4327(15) . . ?
O15 Mo3 Mo7 89.6281(6) . . ?
O15 Mo3 O3 165.247(2) . . ?
O15 Mo3 O5 96.9930(12) . . ?
O15 Mo3 O7 100.0300(11) . . ?
O15 Mo3 O10 97.6679(8) . . ?
O18 Mo3 Mo1 87.5350(10) . . ?
O18 Mo3 Mo5 117.5622(10) . . ?
O18 Mo3 Mo7 124.9097(8) . . ?
O18 Mo3 O3 88.4303(11) . . ?
O18 Mo3 O5 154.8499(8) . . ?
O18 Mo3 O7 90.5613(12) . . ?
O18 Mo3 O10 100.1995(10) . . ?
O18 Mo3 O15 104.717(2) . . ?
Mo5 Mo4 Mo2 61.3806(6) . . ?
Mo7 Mo4 Mo2 124.1678(5) . . ?
Mo7 Mo4 Mo5 63.0746(6) . . ?
O4 Mo4 Mo2 43.2282(6) . . ?
O4 Mo4 Mo5 31.3129(10) . . ?
O4 Mo4 Mo7 88.2713(9) . . ?
O5 Mo4 Mo2 89.5635(8) . . ?
O5 Mo4 Mo5 41.2002(9) . . ?
O5 Mo4 Mo7 41.8453(6) . . ?
O5 Mo4 O4 72.3667(11) . . ?
O8 Mo4 Mo2 129.6207(6) . . ?
O8 Mo4 Mo5 132.6157(17) . . ?
O8 Mo4 Mo7 86.0446(15) . . ?
O8 Mo4 O4 161.2900(15) . . ?
O8 Mo4 O5 91.7263(18) . . ?
O13 Mo4 Mo2 129.0028(8) . . ?
O13 Mo4 Mo5 75.4173(4) . . ?
O13 Mo4 Mo7 33.8961(11) . . ?
O13 Mo4 O4 85.8165(7) . . ?
O13 Mo4 O5 72.8123(10) . . ?
O13 Mo4 O8 99.0935(16) . . ?
O16 Mo4 Mo2 33.1440(9) . . ?
O16 Mo4 Mo5 80.2934(4) . . ?
O16 Mo4 Mo7 130.1035(12) . . ?
O16 Mo4 O4 73.7314(8) . . ?
O16 Mo4 O5 88.2727(10) . . ?
O16 Mo4 O8 96.5473(9) . . ?
O16 Mo4 O13 155.6900(6) . . ?
O23 Mo4 Mo2 88.0956(15) . . ?
O23 Mo4 Mo5 123.8955(13) . . ?
O23 Mo4 Mo7 128.7024(6) . . ?
O23 Mo4 O4 94.0898(17) . . ?
O23 Mo4 O5 162.1370(8) . . ?
O23 Mo4 O8 103.3689(11) . . ?
O23 Mo4 O13 95.1000(11) . . ?
O23 Mo4 O16 99.2584(18) . . ?
Mo2 Mo5 Mo1 77.5717(6) . . ?
Mo3 Mo5 Mo1 57.7007(7) . . ?
Mo3 Mo5 Mo2 103.2914(6) . . ?
Mo4 Mo5 Mo1 103.2030(3) . . ?
Mo4 Mo5 Mo2 56.8239(6) . . ?
Mo4 Mo5 Mo3 75.8447(7) . . ?
Mo6 Mo5 Mo1 56.3696(7) . . ?
Mo6 Mo5 Mo2 56.1169(5) . . ?
Mo6 Mo5 Mo3 113.6496(6) . . ?
Mo6 Mo5 Mo4 112.5911(7) . . ?
Mo7 Mo5 Mo1 112.8097(10) . . ?
Mo7 Mo5 Mo2 111.9584(4) . . ?
Mo7 Mo5 Mo3 55.3940(6) . . ?
Mo7 Mo5 Mo4 55.3599(6) . . ?
Mo7 Mo5 Mo6 163.7583(3) . . ?
O1 Mo5 Mo1 39.6698(9) . . ?
O1 Mo5 Mo2 38.9363(8) . . ?
O1 Mo5 Mo3 84.4151(11) . . ?
O1 Mo5 Mo4 83.3616(4) . . ?
O1 Mo5 Mo6 37.6075(7) . . ?
O1 Mo5 Mo7 126.1617(8) . . ?
O3 Mo5 Mo1 38.1466(8) . . ?
O3 Mo5 Mo2 114.0102(6) . . ?
O3 Mo5 Mo3 39.7319(8) . . ?
O3 Mo5 Mo4 113.6555(10) . . ?
O3 Mo5 Mo6 87.5646(9) . . ?
O3 Mo5 Mo7 88.2698(14) . . ?
O3 Mo5 O1 77.6752(10) . . ?
O4 Mo5 Mo1 113.1074(5) . . ?
O4 Mo5 Mo2 37.7360(5) . . ?
O4 Mo5 Mo3 111.5758(10) . . ?
O4 Mo5 Mo4 37.4847(10) . . ?
O4 Mo5 Mo6 87.6986(12) . . ?
O4 Mo5 Mo7 86.2371(9) . . ?
O4 Mo5 O1 76.4144(9) . . ?
O4 Mo5 O3 143.1001(7) . . ?
O5 Mo5 Mo1 83.7446(7) . . ?
O5 Mo5 Mo2 84.1588(8) . . ?
O5 Mo5 Mo3 37.7412(8) . . ?
O5 Mo5 Mo4 39.1639(9) . . ?
O5 Mo5 Mo6 126.7634(4) . . ?
O5 Mo5 Mo7 37.0263(5) . . ?
O5 Mo5 O1 89.1578(7) . . ?
O5 Mo5 O3 77.3154(13) . . ?
O5 Mo5 O4 76.4875(11) . . ?
O9 Mo5 Mo1 138.6420(19) . . ?
O9 Mo5 Mo2 139.1702(11) . . ?
O9 Mo5 Mo3 89.4094(16) . . ?
O9 Mo5 Mo4 90.4031(5) . . ?
O9 Mo5 Mo6 150.2674(10) . . ?
O9 Mo5 Mo7 45.9632(8) . . ?
O9 Mo5 O1 172.1248(14) . . ?
O9 Mo5 O3 100.6056(19) . . ?
O9 Mo5 O4 101.4726(10) . . ?
O9 Mo5 O5 82.9681(12) . . ?
O17 Mo5 Mo1 91.0841(7) . . ?
O17 Mo5 Mo2 89.6716(14) . . ?
O17 Mo5 Mo3 141.3913(12) . . ?
O17 Mo5 Mo4 138.3827(18) . . ?
O17 Mo5 Mo6 45.9593(6) . . ?
O17 Mo5 Mo7 150.2192(4) . . ?
O17 Mo5 O1 83.5544(11) . . ?
O17 Mo5 O3 101.7506(11) . . ?
O17 Mo5 O4 100.951(2) . . ?
O17 Mo5 O5 172.6730(9) . . ?
O17 Mo5 O9 104.3171(8) . . ?
Mo2 Mo6 Mo1 82.9148(8) . . ?
Mo5 Mo6 Mo1 61.1694(7) . . ?
Mo5 Mo6 Mo2 61.8051(6) . . ?
O1 Mo6 Mo1 42.6386(9) . . ?
O1 Mo6 Mo2 42.5046(10) . . ?
O1 Mo6 Mo5 39.7443(4) . . ?
O2 Mo6 Mo1 34.9487(7) . . ?
O2 Mo6 Mo2 117.0557(13) . . ?
O2 Mo6 Mo5 75.2715(11) . . ?
O2 Mo6 O1 74.9190(14) . . ?
O12 Mo6 Mo1 93.9959(14) . . ?
O12 Mo6 Mo2 94.4384(5) . . ?
O12 Mo6 Mo5 146.0582(11) . . ?
O12 Mo6 O1 106.3249(9) . . ?
O12 Mo6 O2 97.8868(14) . . ?
O17 Mo6 Mo1 82.5479(11) . . ?
O17 Mo6 Mo2 82.2635(5) . . ?
O17 Mo6 Mo5 29.4146(6) . . ?
O17 Mo6 O1 69.1494(8) . . ?
O17 Mo6 O2 80.9682(12) . . ?
O17 Mo6 O12 175.4728(14) . . ?
O20 Mo6 Mo1 134.1702(16) . . ?
O20 Mo6 Mo2 134.9468(14) . . ?
O20 Mo6 Mo5 108.9846(8) . . ?
O20 Mo6 O1 148.7289(10) . . ?
O20 Mo6 O2 100.3017(13) . . ?
O20 Mo6 O12 104.9415(15) . . ?
O20 Mo6 O17 79.5829(8) . . ?
O21 Mo6 Mo1 117.2275(11) . . ?
O21 Mo6 Mo2 35.3168(9) . . ?
O21 Mo6 Mo5 75.6313(10) . . ?
O21 Mo6 O1 74.8759(12) . . ?
O21 Mo6 O2 148.3831(17) . . ?
O21 Mo6 O12 99.3191(15) . . ?
O21 Mo6 O17 79.7951(8) . . ?
O21 Mo6 O20 100.6010(17) . . ?
Mo4 Mo7 Mo3 82.1627(6) . . ?
Mo5 Mo7 Mo3 61.6861(7) . . ?
Mo5 Mo7 Mo4 61.5654(6) . . ?
O5 Mo7 Mo3 41.5518(10) . . ?
O5 Mo7 Mo4 42.9912(8) . . ?
O5 Mo7 Mo5 39.9389(6) . . ?
O7 Mo7 Mo3 35.7522(6) . . ?
O7 Mo7 Mo4 116.9784(8) . . ?
O7 Mo7 Mo5 75.5693(11) . . ?
O7 Mo7 O5 74.3253(10) . . ?
O9 Mo7 Mo3 82.1826(6) . . ?
O9 Mo7 Mo4 82.8166(11) . . ?
O9 Mo7 Mo5 29.1169(3) . . ?
O9 Mo7 O5 69.0394(8) . . ?
O9 Mo7 O7 79.7956(10) . . ?
O13 Mo7 Mo3 116.0292(9) . . ?
O13 Mo7 Mo4 34.8804(5) . . ?
O13 Mo7 Mo5 74.6265(11) . . ?
O13 Mo7 O5 74.8306(13) . . ?
O13 Mo7 O7 147.6504(14) . . ?
O13 Mo7 O9 80.3260(14) . . ?
O14 Mo7 Mo3 94.8027(10) . . ?
O14 Mo7 Mo4 94.1075(10) . . ?
O14 Mo7 Mo5 146.8257(5) . . ?
O14 Mo7 O5 106.9041(7) . . ?
O14 Mo7 O7 99.3584(19) . . ?
O14 Mo7 O9 175.9425(7) . . ?
O14 Mo7 O13 98.6727(12) . . ?
O24 Mo7 Mo3 134.9038(11) . . ?
O24 Mo7 Mo4 134.6935(19) . . ?
O24 Mo7 Mo5 108.2771(11) . . ?
O24 Mo7 O5 148.2038(15) . . ?
O24 Mo7 O7 100.2332(12) . . ?
O24 Mo7 O9 79.1669(10) . . ?
O24 Mo7 O13 100.7765(16) . . ?
O24 Mo7 O14 104.8901(14) . . ?
O1W Pd1 O1W 87.9669(11) . 14_345 ?
O2W Pd1 O1W 92.1664(8) 14_345 14_345 ?
O2W Pd1 O1W 92.1664(8) . . ?
O2W Pd1 O1W 173.3412(9) . 14_345 ?
O2W Pd1 O1W 173.3412(9) 14_345 . ?
O2W Pd1 O2W 88.4727(12) 14_345 . ?
Mo2 O1 Mo1 153.4904(5) . . ?
Mo5 O1 Mo1 99.4723(14) . . ?
Mo5 O1 Mo2 100.8907(9) . . ?
Mo6 O1 Mo1 95.8667(10) . . ?
Mo6 O1 Mo2 96.0458(17) . . ?
Mo6 O1 Mo5 102.6482(7) . . ?
Mo6 O2 Mo1 110.8962(10) . . ?
Mo3 O3 Mo1 92.6106(8) . . ?
Mo5 O3 Mo1 110.2875(17) . . ?
Mo5 O3 Mo3 108.9756(8) . . ?
Mo4 O4 Mo2 93.4567(6) . . ?
Mo5 O4 Mo2 110.6951(8) . . ?
Mo5 O4 Mo4 111.2025(19) . . ?
Mo4 O5 Mo3 152.6077(6) . . ?
Mo5 O5 Mo3 101.4829(9) . . ?
Mo5 O5 Mo4 99.6359(16) . . ?
Mo7 O5 Mo3 96.8527(16) . . ?
Mo7 O5 Mo4 95.1635(9) . . ?
Mo7 O5 Mo5 103.0348(6) . . ?
Mo7 O7 Mo3 109.8970(14) . . ?
Mo7 O9 Mo5 104.9199(8) . . ?
Mo3 O10 Mo1 116.0419(6) . . ?
Mo7 O13 Mo4 111.2235(12) . . ?
Mo4 O16 Mo2 113.9943(10) . . ?
Mo6 O17 Mo5 104.6261(6) . . ?
Mo6 O21 Mo2 110.9620(18) . . ?
H1Wa O1W Pd1 110.650(2) . 14_345 ?
H1Wb O1W Pd1 109.901(3) . 14_345 ?
H1Wb O1W H1Wa 104.5024(19) . . ?
H2Wa O2W Pd1 108.129(3) . 14_345 ?
H2Wb O2W Pd1 110.0361(14) . 14_345 ?
H2Wb O2W H2Wa 104.4824(17) . . ?
H3wb o3w H3wa 109.489(3) . . ?
H4wb o4w H4wa 109.4832(19) . . ?
H5wb o5w H5wa 104.494(3) . . ?
H6wb o6w H6wa 109.471(3) . . ?
H7wb o7w H7wa 109.470(4) . . ?
H9wb o9w H9wa 109.471(2) . . ?
H10b o10w H10a 109.4712(9) . . ?

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_compound2'
_database_code_depnum_ccdc_archive 'CCDC 2042535'
loop_
_audit_author_name
_audit_author_address
'Hai Fu'
;CCUT china
China
;
_audit_update_record             
;
2020-11-05 deposited with the CCDC.	2021-01-07 downloaded from the CCDC.
;
_audit_creation_date             2020-11-04
_audit_creation_method           
;
Olex2 1.2
(compiled 2014.09.19 svn.r3010 for OlexSys, GUI svn.r4874)
;
_chemical_formula_moiety         'Mo7 O24, 2(H8 O4 Pd), 3(H2 O)'
_chemical_formula_sum            'H22 Mo7 O35 Pd2'
_chemical_formula_weight         1466.50
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_Cromer_Mann_a1
_atom_type_scat_Cromer_Mann_a2
_atom_type_scat_Cromer_Mann_a3
_atom_type_scat_Cromer_Mann_a4
_atom_type_scat_Cromer_Mann_b1
_atom_type_scat_Cromer_Mann_b2
_atom_type_scat_Cromer_Mann_b3
_atom_type_scat_Cromer_Mann_b4
_atom_type_scat_Cromer_Mann_c
_atom_type_scat_source
_atom_type_scat_dispersion_source
H 0.00000 0.00000 0.49300 0.32291 0.14019 0.04081 10.51090 26.12570 3.14236
57.79970 0.0030380000826
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Mo -1.68402 0.70339 3.70250 17.23560 12.88760 3.74290 0.27720 1.09580 11.00400
61.65840 4.38749980927
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
O 0.01158 0.00611 3.04850 2.28680 1.54630 0.86700 13.27710 5.70110 0.32390
32.90890 0.250800013542
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Pd -0.98845 1.01473 19.33190 15.50170 5.29537 0.60584 0.69866 7.98929 25.20520
76.89860 5.26593017578
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'

_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_H-M_alt        'C 1 2/c 1'
_space_group_name_Hall           '-C 2yc'
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,y,-z+1/2
3 -x,-y,-z
4 x,-y,z-1/2
5 x+1/2,y+1/2,z
6 -x+1/2,y+1/2,-z+1/2
7 -x+1/2,-y+1/2,-z
8 x+1/2,-y+1/2,z-1/2

_symmetry_Int_Tables_number      15
_cell_length_a                   31.524(6)
_cell_length_b                   10.224(2)
_cell_length_c                   19.965(4)
_cell_angle_alpha                90
_cell_angle_beta                 108.653(5)
_cell_angle_gamma                90
_cell_volume                     6097(2)
_cell_formula_units_Z            8
_cell_measurement_reflns_used    9859
_cell_measurement_theta_max      28.409
_cell_measurement_theta_min      3.159
_exptl_absorpt_coefficient_mu    4.051
_exptl_absorpt_correction_type   none
_exptl_crystal_density_diffrn    3.1953
_exptl_crystal_F_000             5394.8038
_diffrn_reflns_av_R_equivalents  0.0845
_diffrn_reflns_av_unetI/netI     0.0597
_diffrn_reflns_limit_h_max       41
_diffrn_reflns_limit_h_min       -42
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            41973
_diffrn_reflns_theta_full        24.9979
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         2.73
_diffrn_measured_fraction_theta_full 0.9953
_diffrn_measured_fraction_theta_max 0.9953
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_reflns_Friedel_coverage         0.0
_reflns_limit_h_max              35
_reflns_limit_h_min              -37
_reflns_limit_k_max              12
_reflns_limit_k_min              0
_reflns_limit_l_max              23
_reflns_limit_l_min              0
_reflns_number_gt                5004
_reflns_number_total             5348
_reflns_threshold_expression     I>=2u(I)
_computing_cell_refinement       'SAINT v8.37A (Bruker, 2015)'
_computing_data_reduction        'SAINT v8.37A (Bruker, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'olex2.refine (Bourhis et al., 2013)'
_refine_diff_density_max         5.5439
_refine_diff_density_min         -2.3214
_refine_diff_density_rms         0.5403
_refine_ls_d_res_high            0.8409
_refine_ls_d_res_low             7.4671
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_goodness_of_fit_ref   1.0234
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_constraints    36
_refine_ls_number_parameters     332
_refine_ls_number_reflns         5348
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0801
_refine_ls_R_factor_gt           0.0750
_refine_ls_restrained_S_all      1.0234
_refine_ls_shift/su_max          0.0034
_refine_ls_shift/su_mean         0.0001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0000P)²+1704.0167P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1655
_refine_ls_wR_factor_ref         0.1682
_olex2_refinement_description    
;
1. Fixed Uiso
 At 1.5 times of:
  All O(H,H) groups
2. Others
 Fixed Sof: H1Wa(0.5) H1Wb(0.5) H10a(0.5) H10b(0.5)
3.a Free rotating group:
 O1W(H1Wa,H1Wb), O10W(H10a,H10b), O11W(H11a,H11b), O12W(H12a,H12b)
3.b Rotating group:
 O9W(H9Wa,H9Wb), O8W(H8Wa,H8Wb), O7W(H7Wa,H7Wb), O6W(H6Wa,H6Wb), O5W(H5Wa,
 H5Wb), O4W(H4Wa,H4Wb), O3W(H3Wa,H3Wb), O2W(H2Wa,H2Wb)
;
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Mo1 Mo 0.1052687(6) 0.5390760(6) 0.3262582(6) 0.01054(16) Uani 1.000000 1 . . .
Mo2 Mo 0.1677726(6) 0.2640568(6) 0.3753683(6) 0.00860(15) Uani 1.000000 1 . . .
Mo3 Mo 0.0914174(6) 0.0192440(6) 0.3223205(6) 0.01225(16) Uani 1.000000 1 . . .
Mo4 Mo 0.1107264(6) 0.2047182(6) 0.2012294(6) 0.01282(16) Uani 1.000000 1 . . .
Mo6 Mo 0.1702207(6) 0.4618533(6) 0.2385009(6) 0.01294(16) Uani 1.000000 1 . . .
Mo7 Mo 0.0847411(6) 0.3507233(6) 0.4444594(6) 0.01057(16) Uani 1.000000 1 . . .
Pd2 Pd 0.2311778(6) 0.6738074(6) 0.5749470(6) 0.01747(16) Uani 1.000000 1 . . .
Mo9 Mo 0.1316874(6) 0.0739047(6) 0.4885940(6) 0.01194(16) Uani 1.000000 1 . . .
Pd1 Pd 0.0222793(6) 0.7686377(6) 0.0869551(6) 0.01323(15) Uani 1.000000 1 . . .
O1 O 0.1051561(6) 0.1879973(6) 0.3919703(6) 0.0086(2) Uani 1.000000 1 . . .
O2 O 0.1222401(6) 0.3637545(6) 0.2771883(6) 0.0121(2) Uani 1.000000 1 . . .
O3 O 0.1459974(6) 0.4126592(6) 0.4129450(6) 0.0113(2) Uani 1.000000 1 . . .
O1W O 0.0 0.7657459(6) 0.25 0.0240469(6) Uiso 1.000000 2 S T P
H1Wa H -0.008335946(16) 0.8352104(6) 0.22601004(2) 0.0360704(9) Uiso 0.500000 1
G . .
H1Wb H -0.024115498(9) 0.7237930(6) 0.24487960(3) 0.0360704(9) Uiso 0.500000 1
G . .
O5 O 0.1297131(6) 0.2494511(6) 0.5205285(6) 0.0157(2) Uani 1.000000 1 . . .
O6 O 0.0615617(6) 0.4336883(6) 0.3530257(6) 0.0103(2) Uani 1.000000 1 . . .
O7 O 0.1332723(6) -0.0394111(6) 0.4139074(6) 0.0153(2) Uani 1.000000 1 . . .
O8 O 0.1501225(6) 0.1237265(6) 0.3123074(6) 0.0185(2) Uani 1.000000 1 . . .
O9 O 0.0362580(6) 0.2705821(6) 0.4421552(6) 0.0143(2) Uani 1.000000 1 . . .
O10 O 0.0853170(6) 0.0124529(6) 0.5040906(6) 0.0229(2) Uani 1.000000 1 . . .
O11 O 0.0410701(6) -0.0165155(6) 0.3342452(6) 0.0243(2) Uani 1.000000 1 . . .
O12 O 0.0894548(6) 0.4914196(6) 0.4962986(6) 0.0232(2) Uani 1.000000 1 . . .
O13 O 0.1618151(6) 0.5776367(6) 0.3092647(6) 0.0141218(6) Uiso 1.000000 1 . . .
O14 O 0.1692796(6) 0.2812290(6) 0.2051570(6) 0.0188(2) Uani 1.000000 1 . . .
O15 O 0.2098898(6) 0.3401962(6) 0.3492034(6) 0.0201(2) Uani 1.000000 1 . . .
O16 O 0.0669291(6) 0.5901630(6) 0.2466936(6) 0.0194(2) Uani 1.000000 1 . . .
O17 O 0.0678653(6) 0.1371741(6) 0.2430624(6) 0.0149(2) Uani 1.000000 1 . . .
O18 O 0.1344289(6) 0.5389630(6) 0.1666875(6) 0.0319(2) Uani 1.000000 1 . . .
O19 O 0.1094238(6) 0.6662337(6) 0.3840374(6) 0.0208(2) Uani 1.000000 1 . . .
O20 O 0.0741984(6) 0.2860720(6) 0.1317032(6) 0.0275(2) Uani 1.000000 1 . . .
O21 O 0.1969377(6) 0.1816270(6) 0.4525486(6) 0.0196394(6) Uiso 1.000000 1 . . .
O22 O 0.2246568(6) 0.5029155(6) 0.2406772(6) 0.0212763(6) Uiso 1.000000 1 . . .
O23 O 0.1783091(6) 0.0184582(6) 0.5547384(6) 0.0240536(6) Uiso 1.000000 1 . . .
O4 O 0.1226921(6) 0.0611148(6) 0.1649989(6) 0.0260497(6) Uiso 1.000000 1 . . .
O24 O 0.1014501(6) -0.1109133(6) 0.2764247(6) 0.0236647(6) Uiso 1.000000 1 . .
.
O9W O 0.0895741(6) 0.7835087(6) 0.1394426(6) 0.0346079(6) Uiso 1.000000 1 . . .
H9Wa H 0.0989321(6) 0.8579851(6) 0.1314275(6) 0.0519119(9) Uiso 1.000000 1 GR .
.
H9Wb H 0.1039864(6) 0.7291878(6) 0.1227735(6) 0.0519119(9) Uiso 1.000000 1 GR .
.
O8W O 0.0184803(6) 0.9691559(6) 0.0878193(6) 0.0373868(6) Uiso 1.000000 1 . . .
H8Wa H 0.0408880(6) 1.0020132(6) 0.0789844(6) 0.0560802(9) Uiso 1.000000 1 GR .
.
H8Wb H 0.0214622(6) 0.9936947(6) 0.1297534(6) 0.0560802(9) Uiso 1.000000 1 GR .
.
O10W O 0.0 0.2990195(6) 0.25 0.0470497(6) Uiso 1.000000 2 S T P
H10a H -0.013468234(14) 0.3195746(6) 0.27919472(2) 0.0705746(9) Uiso 0.500000 1
G . .
H10b H -0.011559113(15) 0.3482019(6) 0.214516325(16) 0.0705746(9) Uiso 0.500000
1 G . .
O7W O 0.2295793(6) 0.8191814(6) 0.6440375(6) 0.0359637(6) Uiso 1.000000 1 . . .
H7Wa H 0.2560216(6) 0.8456873(6) 0.6653781(6) 0.0539455(9) Uiso 1.000000 1 GR .
.
H7Wb H 0.2206768(6) 0.7872498(6) 0.6765251(6) 0.0539455(9) Uiso 1.000000 1 GR .
.
O6W O 0.0289105(6) 0.5669673(6) 0.0923895(6) 0.0432087(6) Uiso 1.000000 1 . . .
H6Wa H 0.0389855(6) 0.5419798(6) 0.0597688(6) 0.0648130(9) Uiso 1.000000 1 GR .
.
H6Wb H 0.0031838(6) 0.5318073(6) 0.0821636(6) 0.0648130(9) Uiso 1.000000 1 GR .
.
O11W O 0.1953998(6) -0.1071917(6) 0.2311927(6) 0.0407511(6) Uiso 1.000000 1 . .
.
H11a H 0.1686940(6) -0.0827758(6) 0.2099258(6) 0.0611267(9) Uiso 1.000000 1 G .
.
H11b H 0.2000881(6) -0.1683600(6) 0.2055981(6) 0.0611267(9) Uiso 1.000000 1 G .
.
O5W O 0.2984261(6) 0.6658513(6) 0.6208145(6) 0.0476142(6) Uiso 1.000000 1 . . .
H5Wa H 0.3093549(6) 0.7425614(6) 0.6278893(6) 0.0714213(9) Uiso 1.000000 1 GR .
.
H5Wb H 0.3097634(6) 0.6322559(6) 0.5914742(6) 0.0714213(9) Uiso 1.000000 1 GR .
.
O4W O 0.2324853(6) 0.5305931(6) 0.5017154(6) 0.0466433(6) Uiso 1.000000 1 . . .
H4Wa H 0.2582109(6) 0.5282347(6) 0.4965419(6) 0.0699650(9) Uiso 1.000000 1 GR .
.
H4Wb H 0.2148586(6) 0.5517772(6) 0.4611981(6) 0.0699650(9) Uiso 1.000000 1 GR .
.
O3W O -0.0453504(6) 0.7539303(6) 0.0327240(6) 0.0463162(6) Uiso 1.000000 1 . .
.
H3Wa H -0.0549736(6) 0.6788118(6) 0.0390510(6) 0.0694742(9) Uiso 1.000000 1 GR
. .
H3Wb H -0.0496368(6) 0.7577870(6) -0.0114814(6) 0.0694742(9) Uiso 1.000000 1 GR
. .
O12W O 0.2076535(6) 0.2856092(6) 0.6339127(6) 0.0465716(6) Uiso 1.000000 1 . .
.
H12a H 0.1988398(6) 0.2077362(6) 0.6364319(6) 0.0698574(9) Uiso 1.000000 1 G .
.
H12b H 0.1963326(6) 0.3059027(6) 0.5905439(6) 0.0698574(9) Uiso 1.000000 1 G .
.
O2W O 0.1625299(6) 0.6884822(6) 0.5365882(6) 0.0557865(6) Uiso 1.000000 1 . . .
H2Wa H 0.1550244(6) 0.7582423(6) 0.5530513(6) 0.0836797(9) Uiso 1.000000 1 GR .
.
H2Wb H 0.1508659(6) 0.6274414(6) 0.5537385(6) 0.0836797(9) Uiso 1.000000 1 GR .
.


loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 Mo2 3.3932(5) . ?
Mo1 Mo6 3.1907(4) . ?
Mo1 Mo7 3.2670(4) . ?
Mo1 O2 2.1896(3) . ?
Mo1 O3 2.2120(3) . ?
Mo1 O6 1.9535(2) . ?
Mo1 O13 1.9583(3) . ?
Mo1 O16 1.7404(3) . ?
Mo1 O19 1.7150(2) . ?
Mo2 Mo3 3.3984(5) . ?
Mo2 Mo4 3.4191(6) . ?
Mo2 Mo6 3.4202(5) . ?
Mo2 Mo7 3.4422(5) . ?
Mo2 Mo9 3.4393(4) . ?
Mo2 O1 2.2427(4) . ?
Mo2 O2 2.2676(3) . ?
Mo2 O3 1.9162(3) . ?
Mo2 O8 1.8722(3) . ?
Mo2 O15 1.7565(2) . ?
Mo2 O21 1.7389(2) . ?
Mo3 Mo4 3.2791(4) . ?
Mo3 Mo9 3.2014(6) . ?
Mo3 O1 2.1709(3) . ?
Mo3 O7 1.9751(3) . ?
Mo3 O8 2.2006(3) . ?
Mo3 O11 1.7179(3) . ?
Mo3 O17 1.9384(3) . ?
Mo3 O24 1.7017(2) . ?
Mo4 Mo6 3.1764(5) . ?
Mo4 O2 2.1733(3) . ?
Mo4 O8 2.3205(4) . ?
Mo4 O14 1.9831(3) . ?
Mo4 O17 1.9292(3) . ?
Mo4 O20 1.7094(2) . ?
Mo4 O4 1.7308(3) . ?
Mo6 O2 2.1535(3) . ?
Mo6 O13 1.9254(3) . ?
Mo6 O14 1.9600(3) . ?
Mo6 O15 2.4956(4) . ?
Mo6 O18 1.7075(2) . ?
Mo6 O22 1.7536(3) . ?
Mo7 Mo9 3.1847(5) . ?
Mo7 O1 2.1706(3) . ?
Mo7 O3 2.3028(4) . ?
Mo7 O5 2.0028(2) . ?
Mo7 O6 1.9320(3) . ?
Mo7 O9 1.7218(3) . ?
Mo7 O12 1.7504(3) . ?
Pd2 O7W 2.0393(3) . ?
Pd2 O5W 2.0243(4) . ?
Pd2 O4W 2.0789(3) . ?
Pd2 O2W 2.0572(4) . ?
Mo9 O1 2.1794(3) . ?
Mo9 O5 1.9123(3) . ?
Mo9 O7 1.9015(3) . ?
Mo9 O10 1.7078(3) . ?
Mo9 O21 2.6285(4) . ?
Mo9 O23 1.7274(2) . ?
Pd1 O9W 2.0493(4) . ?
Pd1 O8W 2.0539(4) . ?
Pd1 O6W 2.0717(4) . ?
Pd1 O3W 2.0649(4) . ?
O1W H1Wa 0.8499 . ?
O1W H1Wa 0.8499 2 ?
O1W H1Wb 0.8501 . ?
O1W H1Wb 0.8501 2 ?
H1Wa H1Wa 0.93372(17) 2 ?
O9W H9Wa 0.8501 . ?
O9W H9Wb 0.8499 . ?
O8W H8Wa 0.8501 . ?
O8W H8Wb 0.8499 . ?
O10W H10a 0.8500 2 ?
O10W H10a 0.8500 . ?
O10W H10b 0.8499 2 ?
O10W H10b 0.8499 . ?
H10a H10b 0.81273(14) 2 ?
O7W H7Wa 0.8501 . ?
O7W H7Wb 0.8500 . ?
O6W H6Wa 0.8501 . ?
O6W H6Wb 0.8501 . ?
O11W H11a 0.8501 . ?
O11W H11b 0.8499 . ?
O5W H5Wa 0.8500 . ?
O5W H5Wb 0.8502 . ?
O4W H4Wa 0.8500 . ?
O4W H4Wb 0.8500 . ?
O3W H3Wa 0.8499 . ?
O3W H3Wb 0.8500 . ?
O12W H12a 0.8500 . ?
O12W H12b 0.8500 . ?
O2W H2Wa 0.8500 . ?
O2W H2Wb 0.8500 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Mo6 Mo1 Mo2 62.5044(4) . . ?
Mo7 Mo1 Mo2 62.2067(4) . . ?
Mo7 Mo1 Mo6 124.1242(4) . . ?
O2 Mo1 Mo2 41.2832(4) . . ?
O2 Mo1 Mo6 42.2839(5) . . ?
O2 Mo1 Mo7 88.5039(5) . . ?
O3 Mo1 Mo2 31.9671(4) . . ?
O3 Mo1 Mo6 88.3522(7) . . ?
O3 Mo1 Mo7 44.7577(6) . . ?
O3 Mo1 O2 73.0242(5) . . ?
O6 Mo1 Mo2 81.9003(5) . . ?
O6 Mo1 Mo6 130.2720(5) . . ?
O6 Mo1 Mo7 32.5698(5) . . ?
O6 Mo1 O2 88.0259(6) . . ?
O6 Mo1 O3 75.3659(7) . . ?
O13 Mo1 Mo2 74.9446(6) . . ?
O13 Mo1 Mo6 34.4219(4) . . ?
O13 Mo1 Mo7 130.1953(6) . . ?
O13 Mo1 O2 73.8026(7) . . ?
O13 Mo1 O3 85.4376(8) . . ?
O13 Mo1 O6 156.8104(7) . . ?
O16 Mo1 Mo2 132.9998(6) . . ?
O16 Mo1 Mo6 87.3244(8) . . ?
O16 Mo1 Mo7 126.5879(10) . . ?
O16 Mo1 O2 92.0062(7) . . ?
O16 Mo1 O3 161.6917(5) . . ?
O16 Mo1 O6 94.0459(10) . . ?
O16 Mo1 O13 100.7392(10) . . ?
O19 Mo1 Mo2 121.4252(7) . . ?
O19 Mo1 Mo6 129.2391(10) . . ?
O19 Mo1 Mo7 87.1955(7) . . ?
O19 Mo1 O2 160.8173(10) . . ?
O19 Mo1 O3 90.9317(6) . . ?
O19 Mo1 O6 98.2149(10) . . ?
O19 Mo1 O13 94.9342(9) . . ?
O19 Mo1 O16 105.5340(7) . . ?
Mo3 Mo2 Mo1 103.4308(6) . . ?
Mo4 Mo2 Mo1 77.5983(4) . . ?
Mo4 Mo2 Mo3 57.4979(3) . . ?
Mo6 Mo2 Mo1 55.8467(4) . . ?
Mo6 Mo2 Mo3 112.4070(4) . . ?
Mo6 Mo2 Mo4 55.3472(4) . . ?
Mo7 Mo2 Mo1 57.0976(4) . . ?
Mo7 Mo2 Mo3 76.1664(5) . . ?
Mo7 Mo2 Mo4 103.4803(6) . . ?
Mo7 Mo2 Mo6 112.4796(5) . . ?
Mo9 Mo2 Mo1 112.0086(6) . . ?
Mo9 Mo2 Mo3 55.8301(4) . . ?
Mo9 Mo2 Mo4 113.0236(5) . . ?
Mo9 Mo2 Mo6 162.9599(7) . . ?
Mo9 Mo2 Mo7 55.1338(4) . . ?
O1 Mo2 Mo1 82.6929(6) . . ?
O1 Mo2 Mo3 38.8798(4) . . ?
O1 Mo2 Mo4 83.5246(6) . . ?
O1 Mo2 Mo6 124.6772(6) . . ?
O1 Mo2 Mo7 37.9978(4) . . ?
O1 Mo2 Mo9 38.2855(4) . . ?
O2 Mo2 Mo1 39.5747(4) . . ?
O2 Mo2 Mo3 82.6589(5) . . ?
O2 Mo2 Mo4 38.6553(3) . . ?
O2 Mo2 Mo6 38.1262(6) . . ?
O2 Mo2 Mo7 83.0203(7) . . ?
O2 Mo2 Mo9 124.8399(9) . . ?
O2 Mo2 O1 86.5546(8) . . ?
O3 Mo2 Mo1 37.6743(4) . . ?
O3 Mo2 Mo3 113.5305(9) . . ?
O3 Mo2 Mo4 113.6429(6) . . ?
O3 Mo2 Mo6 86.9323(5) . . ?
O3 Mo2 Mo7 39.2365(6) . . ?
O3 Mo2 Mo9 87.4553(7) . . ?
O3 Mo2 O1 76.9722(8) . . ?
O3 Mo2 O2 77.0015(6) . . ?
O8 Mo2 Mo1 114.8639(7) . . ?
O8 Mo2 Mo3 36.6297(7) . . ?
O8 Mo2 Mo4 39.9737(4) . . ?
O8 Mo2 Mo6 89.6325(6) . . ?
O8 Mo2 Mo7 111.4832(9) . . ?
O8 Mo2 Mo9 85.3670(6) . . ?
O8 Mo2 O1 75.3665(8) . . ?
O8 Mo2 O2 78.0717(6) . . ?
O8 Mo2 O3 143.5403(12) . . ?
O15 Mo2 Mo1 88.3466(6) . . ?
O15 Mo2 Mo3 139.5615(7) . . ?
O15 Mo2 Mo4 88.7380(6) . . ?
O15 Mo2 Mo6 44.6014(5) . . ?
O15 Mo2 Mo7 138.5125(5) . . ?
O15 Mo2 Mo9 152.4190(7) . . ?
O15 Mo2 O1 169.2292(7) . . ?
O15 Mo2 O2 82.7269(7) . . ?
O15 Mo2 O3 99.4734(7) . . ?
O15 Mo2 O8 103.2935(10) . . ?
O21 Mo2 Mo1 138.6976(7) . . ?
O21 Mo2 Mo3 92.3089(6) . . ?
O21 Mo2 Mo4 140.5493(4) . . ?
O21 Mo2 Mo6 148.6411(11) . . ?
O21 Mo2 Mo7 91.3712(9) . . ?
O21 Mo2 Mo9 48.3853(8) . . ?
O21 Mo2 O1 86.6686(9) . . ?
O21 Mo2 O2 173.2104(13) . . ?
O21 Mo2 O3 101.0336(8) . . ?
O21 Mo2 O8 100.5874(5) . . ?
O21 Mo2 O15 104.0406(11) . . ?
Mo4 Mo3 Mo2 61.5683(4) . . ?
Mo9 Mo3 Mo2 62.7312(4) . . ?
Mo9 Mo3 Mo4 123.9210(5) . . ?
O1 Mo3 Mo2 40.4245(6) . . ?
O1 Mo3 Mo4 88.0890(5) . . ?
O1 Mo3 Mo9 42.7191(3) . . ?
O7 Mo3 Mo2 74.8248(5) . . ?
O7 Mo3 Mo4 129.1684(9) . . ?
O7 Mo3 Mo9 33.5934(4) . . ?
O7 Mo3 O1 73.1963(5) . . ?
O8 Mo3 Mo2 30.5041(4) . . ?
O8 Mo3 Mo4 44.9679(4) . . ?
O8 Mo3 Mo9 86.7544(6) . . ?
O8 Mo3 O1 70.7999(7) . . ?
O8 Mo3 O7 84.2199(8) . . ?
O11 Mo3 Mo2 135.0100(6) . . ?
O11 Mo3 Mo4 128.5242(7) . . ?
O11 Mo3 Mo9 88.3358(7) . . ?
O11 Mo3 O1 94.8323(9) . . ?
O11 Mo3 O7 100.3884(9) . . ?
O11 Mo3 O8 163.1368(6) . . ?
O17 Mo3 Mo2 81.0547(5) . . ?
O17 Mo3 Mo4 31.9388(7) . . ?
O17 Mo3 Mo9 131.2446(4) . . ?
O17 Mo3 O1 88.5363(5) . . ?
O17 Mo3 O7 155.8794(8) . . ?
O17 Mo3 O8 74.7862(7) . . ?
O17 Mo3 O11 96.6544(9) . . ?
O24 Mo3 Mo2 120.5727(11) . . ?
O24 Mo3 Mo4 86.8406(7) . . ?
O24 Mo3 Mo9 127.9183(6) . . ?
O24 Mo3 O1 158.9134(13) . . ?
O24 Mo3 O7 94.4124(7) . . ?
O24 Mo3 O8 91.3824(10) . . ?
O24 Mo3 O11 104.3167(8) . . ?
O24 Mo3 O17 97.7831(8) . . ?
Mo3 Mo4 Mo2 60.9338(4) . . ?
Mo6 Mo4 Mo2 62.3426(3) . . ?
Mo6 Mo4 Mo3 122.7383(5) . . ?
O2 Mo4 Mo2 40.6719(4) . . ?
O2 Mo4 Mo3 86.9677(6) . . ?
O2 Mo4 Mo6 42.5255(6) . . ?
O8 Mo4 Mo2 31.2198(3) . . ?
O8 Mo4 Mo3 42.0825(6) . . ?
O8 Mo4 Mo6 88.6250(5) . . ?
O8 Mo4 O2 71.4076(5) . . ?
O14 Mo4 Mo2 73.1186(6) . . ?
O14 Mo4 Mo3 126.0773(6) . . ?
O14 Mo4 Mo6 36.0889(4) . . ?
O14 Mo4 O2 74.4371(7) . . ?
O14 Mo4 O8 84.0352(7) . . ?
O17 Mo4 Mo2 80.6017(6) . . ?
O17 Mo4 Mo3 32.1088(5) . . ?
O17 Mo4 Mo6 129.6151(6) . . ?
O17 Mo4 O2 87.1037(8) . . ?
O17 Mo4 O8 72.1443(7) . . ?
O17 Mo4 O14 153.6361(8) . . ?
O20 Mo4 Mo2 137.5623(5) . . ?
O20 Mo4 Mo3 130.1195(11) . . ?
O20 Mo4 Mo6 88.9383(5) . . ?
O20 Mo4 O2 96.9740(6) . . ?
O20 Mo4 O8 164.8671(11) . . ?
O20 Mo4 O14 102.5290(9) . . ?
O20 Mo4 O17 98.1954(11) . . ?
O4 Mo4 Mo2 117.4800(6) . . ?
O4 Mo4 Mo3 86.2314(6) . . ?
O4 Mo4 Mo6 127.4940(11) . . ?
O4 Mo4 O2 156.3750(10) . . ?
O4 Mo4 O8 88.5774(6) . . ?
O4 Mo4 O14 91.5241(10) . . ?
O4 Mo4 O17 98.8440(8) . . ?
O4 Mo4 O20 104.6906(8) . . ?
Mo2 Mo6 Mo1 61.6488(4) . . ?
Mo4 Mo6 Mo1 84.1977(6) . . ?
Mo4 Mo6 Mo2 62.3102(4) . . ?
O2 Mo6 Mo1 43.1619(4) . . ?
O2 Mo6 Mo2 40.5486(5) . . ?
O2 Mo6 Mo4 43.0101(4) . . ?
O13 Mo6 Mo1 35.0967(6) . . ?
O13 Mo6 Mo2 74.5530(6) . . ?
O13 Mo6 Mo4 118.1132(9) . . ?
O13 Mo6 O2 75.2761(8) . . ?
O14 Mo6 Mo1 118.4888(8) . . ?
O14 Mo6 Mo2 73.2945(5) . . ?
O14 Mo6 Mo4 36.5824(7) . . ?
O14 Mo6 O2 75.3433(7) . . ?
O14 Mo6 O13 146.9102(9) . . ?
O15 Mo6 Mo1 82.2287(6) . . ?
O15 Mo6 Mo2 29.6185(5) . . ?
O15 Mo6 Mo4 83.4584(4) . . ?
O15 Mo6 O2 70.1665(6) . . ?
O15 Mo6 O13 78.7032(6) . . ?
O15 Mo6 O14 77.2972(5) . . ?
O18 Mo6 Mo1 88.8025(9) . . ?
O18 Mo6 Mo2 140.0123(11) . . ?
O18 Mo6 Mo4 90.1897(7) . . ?
O18 Mo6 O2 99.4918(11) . . ?
O18 Mo6 O13 97.0798(8) . . ?
O18 Mo6 O14 102.4529(7) . . ?
O18 Mo6 O15 169.4738(13) . . ?
O22 Mo6 Mo1 136.2126(6) . . ?
O22 Mo6 Mo2 113.1857(6) . . ?
O22 Mo6 Mo4 134.7267(7) . . ?
O22 Mo6 O2 153.7148(7) . . ?
O22 Mo6 O13 101.4136(8) . . ?
O22 Mo6 O14 98.1839(9) . . ?
O22 Mo6 O15 83.5792(7) . . ?
O22 Mo6 O18 106.7903(10) . . ?
Mo2 Mo7 Mo1 60.6957(4) . . ?
Mo9 Mo7 Mo1 122.8060(7) . . ?
Mo9 Mo7 Mo2 62.3862(4) . . ?
O1 Mo7 Mo1 86.8584(6) . . ?
O1 Mo7 Mo2 39.4988(5) . . ?
O1 Mo7 Mo9 43.0438(4) . . ?
O3 Mo7 Mo1 42.5579(4) . . ?
O3 Mo7 Mo2 31.7567(3) . . ?
O3 Mo7 Mo9 87.9295(6) . . ?
O3 Mo7 O1 71.0233(7) . . ?
O5 Mo7 Mo1 126.6397(10) . . ?
O5 Mo7 Mo2 74.1125(8) . . ?
O5 Mo7 Mo9 34.6309(3) . . ?
O5 Mo7 O1 73.8961(6) . . ?
O5 Mo7 O3 84.1043(9) . . ?
O6 Mo7 Mo1 32.9770(6) . . ?
O6 Mo7 Mo2 80.8298(8) . . ?
O6 Mo7 Mo9 130.8020(6) . . ?
O6 Mo7 O1 87.7789(7) . . ?
O6 Mo7 O3 73.6144(8) . . ?
O6 Mo7 O5 154.8983(13) . . ?
O9 Mo7 Mo1 129.8235(7) . . ?
O9 Mo7 Mo2 130.4731(6) . . ?
O9 Mo7 Mo9 85.0948(5) . . ?
O9 Mo7 O1 91.1519(7) . . ?
O9 Mo7 O3 159.7749(7) . . ?
O9 Mo7 O5 100.4438(7) . . ?
O9 Mo7 O6 96.8595(9) . . ?
O12 Mo7 Mo1 86.7771(6) . . ?
O12 Mo7 Mo2 121.1210(10) . . ?
O12 Mo7 Mo9 128.5075(7) . . ?
O12 Mo7 O1 158.9222(12) . . ?
O12 Mo7 O3 90.8923(8) . . ?
O12 Mo7 O5 94.0604(7) . . ?
O12 Mo7 O6 97.6337(5) . . ?
O12 Mo7 O9 108.2769(12) . . ?
O5W Pd2 O7W 88.4042(7) . . ?
O4W Pd2 O7W 177.9635(6) . . ?
O4W Pd2 O5W 92.0861(8) . . ?
O2W Pd2 O7W 87.0210(8) . . ?
O2W Pd2 O5W 174.9536(9) . . ?
O2W Pd2 O4W 92.5598(7) . . ?
Mo3 Mo9 Mo2 61.4387(4) . . ?
Mo7 Mo9 Mo2 62.4800(4) . . ?
Mo7 Mo9 Mo3 82.7121(4) . . ?
O1 Mo9 Mo2 39.6113(6) . . ?
O1 Mo9 Mo3 42.5133(3) . . ?
O1 Mo9 Mo7 42.8297(4) . . ?
O5 Mo9 Mo2 75.0205(6) . . ?
O5 Mo9 Mo3 117.7216(5) . . ?
O5 Mo9 Mo7 36.5259(4) . . ?
O5 Mo9 O1 75.4403(5) . . ?
O7 Mo9 Mo2 74.4410(6) . . ?
O7 Mo9 Mo3 35.0781(4) . . ?
O7 Mo9 Mo7 116.8003(6) . . ?
O7 Mo9 O1 74.3853(6) . . ?
O7 Mo9 O5 147.6800(8) . . ?
O10 Mo9 Mo2 144.0216(7) . . ?
O10 Mo9 Mo3 92.5869(7) . . ?
O10 Mo9 Mo7 91.6103(7) . . ?
O10 Mo9 O1 104.4105(9) . . ?
O10 Mo9 O5 99.4298(10) . . ?
O10 Mo9 O7 99.0115(8) . . ?
O21 Mo9 Mo2 29.6435(4) . . ?
O21 Mo9 Mo3 82.8032(6) . . ?
O21 Mo9 Mo7 83.5120(5) . . ?
O21 Mo9 O1 69.2533(7) . . ?
O21 Mo9 O5 79.0368(7) . . ?
O21 Mo9 O7 79.7132(8) . . ?
O21 Mo9 O10 173.6606(7) . . ?
O23 Mo9 Mo2 107.9745(10) . . ?
O23 Mo9 Mo3 133.9266(8) . . ?
O23 Mo9 Mo7 135.2050(5) . . ?
O23 Mo9 O1 147.5845(12) . . ?
O23 Mo9 O5 99.4135(7) . . ?
O23 Mo9 O7 99.8026(9) . . ?
O23 Mo9 O10 108.0018(9) . . ?
O23 Mo9 O21 78.3360(9) . . ?
O8W Pd1 O9W 88.5824(6) . . ?
O6W Pd1 O9W 88.6500(7) . . ?
O6W Pd1 O8W 176.4396(7) . . ?
O3W Pd1 O9W 179.1885(10) . . ?
O3W Pd1 O8W 91.3689(7) . . ?
O3W Pd1 O6W 91.4300(6) . . ?
Mo3 O1 Mo2 100.6957(8) . . ?
Mo7 O1 Mo2 102.5034(6) . . ?
Mo7 O1 Mo3 152.7699(11) . . ?
Mo9 O1 Mo2 102.1032(8) . . ?
Mo9 O1 Mo3 94.7676(5) . . ?
Mo9 O1 Mo7 94.1265(7) . . ?
Mo2 O2 Mo1 99.1421(6) . . ?
Mo4 O2 Mo1 156.1358(9) . . ?
Mo4 O2 Mo2 100.6728(5) . . ?
Mo6 O2 Mo1 94.5542(6) . . ?
Mo6 O2 Mo2 101.3252(9) . . ?
Mo6 O2 Mo4 94.4643(8) . . ?
Mo2 O3 Mo1 110.3585(7) . . ?
Mo7 O3 Mo1 92.6845(8) . . ?
Mo7 O3 Mo2 109.0069(7) . . ?
H1Wa O1W H1Wa 66.6400(3) 2 . ?
H1Wb O1W H1Wa 104.5 . . ?
H1Wb O1W H1Wa 104.5 2 2 ?
H1Wb O1W H1Wa 126.4 . 2 ?
H1Wb O1W H1Wa 126.4 2 . ?
H1Wb O1W H1Wb 119.3965(3) 2 . ?
H1Wa H1Wa O1W 56.68002(13) 2 . ?
Mo9 O5 Mo7 108.8433(7) . . ?
Mo7 O6 Mo1 114.4532(10) . . ?
Mo9 O7 Mo3 111.3285(8) . . ?
Mo3 O8 Mo2 112.8662(10) . . ?
Mo4 O8 Mo2 108.8065(5) . . ?
Mo4 O8 Mo3 92.9496(7) . . ?
Mo6 O13 Mo1 110.4814(8) . . ?
Mo6 O14 Mo4 107.3287(10) . . ?
Mo6 O15 Mo2 105.7801(9) . . ?
Mo4 O17 Mo3 115.9524(11) . . ?
Mo9 O21 Mo2 101.9711(10) . . ?
H9Wa O9W Pd1 109.6 . . ?
H9Wb O9W Pd1 110.3 . . ?
H9Wb O9W H9Wa 104.5 . . ?
H8Wa O8W Pd1 109.8 . . ?
H8Wb O8W Pd1 108.3 . . ?
H8Wb O8W H8Wa 104.5 . . ?
H10a O10W H10a 151.37194(13) . 2 ?
H10b O10W H10a 104.5 . . ?
H10b O10W H10a 57.1 . 2 ?
H10b O10W H10a 104.5 2 2 ?
H10b O10W H10a 57.1 2 . ?
H10b O10W H10b 107.4576(3) . 2 ?
H10b H10a O10W 61.43485(16) 2 2 ?
H10a H10b O10W 61.44278(10) 2 2 ?
H7Wa O7W Pd2 109.8 . . ?
H7Wb O7W Pd2 108.8 . . ?
H7Wb O7W H7Wa 104.5 . . ?
H6Wa O6W Pd1 108.4 . . ?
H6Wb O6W Pd1 109.6 . . ?
H6Wb O6W H6Wa 104.5 . . ?
H11b O11W H11a 104.5 . . ?
H5Wa O5W Pd2 110.4 . . ?
H5Wb O5W Pd2 108.3 . . ?
H5Wb O5W H5Wa 104.5 . . ?
H4Wa O4W Pd2 109.9 . . ?
H4Wb O4W Pd2 109.6 . . ?
H4Wb O4W H4Wa 104.5 . . ?
H3Wa O3W Pd1 110.2 . . ?
H3Wb O3W Pd1 109.6 . . ?
H3Wb O3W H3Wa 104.5 . . ?
H12b O12W H12a 104.5 . . ?
H2Wa O2W Pd2 107.9 . . ?
H2Wb O2W Pd2 109.6 . . ?
H2Wb O2W H2Wa 104.5 . . ?

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_compound2
_database_code_depnum_ccdc_archive 'CCDC 2042534'
loop_
_audit_author_name
_audit_author_address
'Hai Fu'
;CCUT china
China
;
_audit_update_record             
;
2020-11-05 deposited with the CCDC.	2021-01-07 downloaded from the CCDC.
;
_audit_creation_date             2020-11-04
_audit_creation_method           
;
Olex2 1.2
(compiled 2014.09.19 svn.r3010 for OlexSys, GUI svn.r4874)
;
_chemical_formula_moiety         'Mo7 O24, 2(H8 O4 Pd), 3(O)'
_chemical_formula_sum            'H16 Mo7 O35 Pd2'
_chemical_formula_weight         1460.46
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_Cromer_Mann_a1
_atom_type_scat_Cromer_Mann_a2
_atom_type_scat_Cromer_Mann_a3
_atom_type_scat_Cromer_Mann_a4
_atom_type_scat_Cromer_Mann_b1
_atom_type_scat_Cromer_Mann_b2
_atom_type_scat_Cromer_Mann_b3
_atom_type_scat_Cromer_Mann_b4
_atom_type_scat_Cromer_Mann_c
_atom_type_scat_source
_atom_type_scat_dispersion_source
H 0.00000 0.00000 0.49300 0.32291 0.14019 0.04081 10.51090 26.12570 3.14236
57.79970 0.0030380000826
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Mo -1.68402 0.70339 3.70250 17.23560 12.88760 3.74290 0.27720 1.09580 11.00400
61.65840 4.38749980927
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
O 0.01158 0.00611 3.04850 2.28680 1.54630 0.86700 13.27710 5.70110 0.32390
32.90890 0.250800013542
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Pd -0.98845 1.01473 19.33190 15.50170 5.29537 0.60584 0.69866 7.98929 25.20520
76.89860 5.26593017578
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'

_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_H-M_alt        'C 1 2/c 1'
_space_group_name_Hall           '-C 2yc'
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,y,-z+1/2
3 -x,-y,-z
4 x,-y,z-1/2
5 x+1/2,y+1/2,z
6 -x+1/2,y+1/2,-z+1/2
7 -x+1/2,-y+1/2,-z
8 x+1/2,-y+1/2,z-1/2

_symmetry_Int_Tables_number      15
_cell_length_a                   29.345(5)
_cell_length_b                   10.1725(17)
_cell_length_c                   19.980(3)
_cell_angle_alpha                90
_cell_angle_beta                 96.914(5)
_cell_angle_gamma                90
_cell_volume                     5920.8(17)
_cell_formula_units_Z            8
_cell_measurement_reflns_used    9632
_cell_measurement_theta_max      28.362
_cell_measurement_theta_min      2.991
_exptl_absorpt_coefficient_mu    4.171
_exptl_absorpt_correction_type   none
_exptl_crystal_density_diffrn    3.2767
_exptl_crystal_F_000             5346.8088
_diffrn_reflns_av_R_equivalents  0.1979
_diffrn_reflns_av_unetI/netI     0.1014
_diffrn_reflns_limit_h_max       38
_diffrn_reflns_limit_h_min       -39
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            61250
_diffrn_reflns_theta_full        24.9980
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         2.89
_diffrn_measured_fraction_theta_full 0.9985
_diffrn_measured_fraction_theta_max 0.9985
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_reflns_Friedel_coverage         0.0
_reflns_limit_h_max              34
_reflns_limit_h_min              -34
_reflns_limit_k_max              12
_reflns_limit_k_min              0
_reflns_limit_l_max              23
_reflns_limit_l_min              0
_reflns_number_gt                4513
_reflns_number_total             5214
_reflns_threshold_expression     I>=2u(I)
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'olex2.refine (Bourhis et al., 2013)'
_refine_diff_density_max         3.4135
_refine_diff_density_min         -3.2785
_refine_diff_density_rms         0.8816
_refine_ls_d_res_high            0.8409
_refine_ls_d_res_low             7.0401
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_goodness_of_fit_ref   1.1157
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_constraints    24
_refine_ls_number_parameters     350
_refine_ls_number_reflns         5214
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0882
_refine_ls_R_factor_gt           0.0670
_refine_ls_restrained_S_all      1.1157
_refine_ls_shift/su_max          2.5352
_refine_ls_shift/su_mean         0.0444
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0096P)²+232.0774P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0885
_refine_ls_wR_factor_ref         0.0947
_olex2_refinement_description    
;
1. Fixed Uiso
 At 1.5 times of:
  All O(H,H) groups
2.a Rotating group:
 O6W(H6Wa,H6Wb), O4W(H4Wa,H4Wb), O8W(H8Wa,H8Wb), O7W(H7Wa,H7Wb), O1W(H1Wa,
 H1Wb), O2W(H2Wa,H2Wb), O3W(H3Wa,H3Wb), O5W(H5Wa,H5Wb)
;
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Mo1 Mo 0.08830(3) 0.47991(8) 0.29103(4) 0.0104(2) Uani 1.000000 1 . . .
Mo2 Mo 0.08655(3) 0.15176(8) 0.41839(4) 0.0119(2) Uani 1.000000 1 . . .
Mo3 Mo 0.12966(3) 0.43544(8) 0.44509(4) 0.0120(2) Uani 1.000000 1 . . .
Mo4 Mo 0.11063(3) -0.03362(8) 0.29448(4) 0.0114(2) Uani 1.000000 1 . . .
Mo5 Mo 0.11792(3) 0.30156(8) 0.16637(4) 0.0124(2) Uani 1.000000 1 . . .
Mo6 Mo 0.17155(3) 0.24860(8) 0.32505(4) 0.00924(19) Uani 1.000000 1 . . .
Pd2 Pd 0.02464(3) -0.25531(8) 0.08119(4) 0.0174(2) Uani 1.000000 1 . . .
Mo8 Mo 0.18146(3) 0.04812(8) 0.19059(4) 0.0144(2) Uani 1.000000 1 . . .
Pd1 Pd 0.21368(3) 0.86810(8) 0.44479(4) 0.0202(2) Uani 1.000000 1 . . .
O1 O 0.0701(2) 0.3583(6) 0.2188(3) 0.0126(14) Uani 1.000000 1 . . .
O2 O 0.1292(2) 0.1418(6) 0.2379(3) 0.0107(14) Uani 1.000000 1 . . .
O3 O 0.1777(2) 0.2230(6) 0.1535(3) 0.0150(15) Uani 1.000000 1 . . .
O4 O 0.1053(2) 0.3166(6) 0.3598(3) 0.0101(14) Uani 1.000000 1 . . .
O5 O 0.1487(2) 0.0973(6) 0.3670(3) 0.0095(14) Uani 1.000000 1 . . .
O6 O 0.1303(2) 0.2589(6) 0.4791(3) 0.0140(14) Uani 1.000000 1 . . .
O7 O 0.1287(2) 0.5478(6) 0.3689(3) 0.0143(15) Uani 1.000000 1 . . .
O8 O 0.2165(2) 0.1747(7) 0.2898(3) 0.0186(16) Uani 1.000000 1 . . .
O9 O 0.1539(2) 0.3854(6) 0.2650(3) 0.0117(14) Uani 1.000000 1 . . .
O10 O 0.0641(2) 0.0689(6) 0.3345(3) 0.0144(14) Uani 1.000000 1 . . .
O11 O 0.0962(2) 0.6152(6) 0.2425(3) 0.0189(16) Uani 1.000000 1 . . .
O12 O 0.0930(3) 0.0135(7) 0.4700(3) 0.0218(17) Uani 1.000000 1 . . .
O13 O 0.0810(2) 0.4922(7) 0.4758(3) 0.0198(16) Uani 1.000000 1 . . .
O14 O 0.1976(2) 0.3308(7) 0.3958(3) 0.0179(15) Uani 1.000000 1 . . .
O15 O 0.0718(2) -0.0825(7) 0.2267(3) 0.0191(16) Uani 1.000000 1 . . .
O16 O 0.1692(2) -0.0735(6) 0.2610(3) 0.0173(15) Uani 1.000000 1 . . .
O17 O 0.1757(2) 0.5049(7) 0.4946(3) 0.0205(16) Uani 1.000000 1 . . .
O18 O 0.0359(2) 0.5056(7) 0.3176(3) 0.0208(16) Uani 1.000000 1 . . .
O19 O 0.1297(3) 0.4500(7) 0.1311(3) 0.0231(17) Uani 1.000000 1 . . .
O8W O 0.0928(3) -0.2675(9) 0.1099(4) 0.044(2) Uiso 1.000000 1 . . .
O21 O 0.1139(3) -0.1608(7) 0.3502(3) 0.0243(17) Uani 1.000000 1 . . .
O12W O 0.0 -0.2581(12) 0.25 0.042(3) Uiso 1.000000 2 S T P
O23 O 0.2389(3) 0.0181(7) 0.1874(4) 0.0300(19) Uani 1.000000 1 . . .
O24 O 0.0832(3) 0.2204(7) 0.1051(3) 0.0270(18) Uani 1.000000 1 . . .
O25 O 0.0358(2) 0.2178(7) 0.4340(3) 0.0257(17) Uani 1.000000 1 . . .
O26 O 0.1539(3) -0.0321(7) 0.1219(3) 0.0284(19) Uani 1.000000 1 . . .
O7W O 0.0315(3) -0.0523(9) 0.0839(5) 0.051(2) Uiso 1.000000 1 . . .
O6W O 0.0220(3) -0.4577(9) 0.0821(4) 0.049(2) Uiso 1.000000 1 . . .
O11W O 0.2915(3) 0.2100(8) 0.4110(4) 0.038(2) Uiso 1.000000 1 . . .
O10W O 0.0 0.2016(12) 0.25 0.044(3) Uiso 1.000000 2 S T P
O5W O 0.2587(3) 0.9327(9) 0.3822(4) 0.046(2) Uiso 1.000000 1 . . .
O4W O -0.0440(3) -0.2432(10) 0.0515(5) 0.051(2) Uiso 1.000000 1 . . .
O3W O 0.2166(3) 1.0427(9) 0.4937(4) 0.049(2) Uiso 1.000000 1 . . .
O2W O 0.1647(3) 0.8061(9) 0.5022(4) 0.048(2) Uiso 1.000000 1 . . .
O9W O 0.1892(3) 0.6527(9) 0.2245(4) 0.049(2) Uiso 1.000000 1 . . .
O1W O 0.2102(4) 0.6910(9) 0.3978(5) 0.056(3) Uiso 1.000000 1 . . .
H6Wa H 0.005(3) -0.4825(9) 0.112(4) 0.073(4) Uiso 1.000000 1 GR . .
H6Wb H 0.0489(5) -0.4882(9) 0.092(5) 0.073(4) Uiso 1.000000 1 GR . .
H4Wa H -0.0551(7) -0.3202(10) 0.047(5) 0.077(4) Uiso 1.000000 1 GR . .
H4Wb H -0.0486(3) -0.202(9) 0.014(3) 0.077(4) Uiso 1.000000 1 GR . .
H8Wa H 0.0976(4) -0.272(10) 0.1526(5) 0.066(3) Uiso 1.000000 1 GR . .
H8Wb H 0.1058(5) -0.200(5) 0.096(4) 0.066(3) Uiso 1.000000 1 GR . .
H7Wa H 0.016(3) -0.0213(13) 0.114(4) 0.076(4) Uiso 1.000000 1 GR . .
H7Wb H 0.021(4) -0.0209(13) 0.0457(17) 0.076(4) Uiso 1.000000 1 GR . .
H1Wa H 0.2367(8) 0.670(6) 0.388(5) 0.084(4) Uiso 1.000000 1 GR . .
H1Wb H 0.192(3) 0.696(3) 0.362(3) 0.084(4) Uiso 1.000000 1 GR . .
H2Wa H 0.1399(12) 0.791(10) 0.4768(7) 0.072(4) Uiso 1.000000 1 GR . .
H2Wb H 0.160(3) 0.866(5) 0.530(4) 0.072(4) Uiso 1.000000 1 GR . .
H3Wa H 0.220(4) 1.0527(9) 0.5363(4) 0.074(4) Uiso 1.000000 1 GR . .
H3Wb H 0.215(4) 1.1176(9) 0.4747(4) 0.074(4) Uiso 1.000000 1 GR . .
H5Wa H 0.254(2) 1.013(3) 0.373(4) 0.069(3) Uiso 1.000000 1 GR . .
H5Wb H 0.255(3) 0.888(7) 0.346(2) 0.069(3) Uiso 1.000000 1 GR . .


loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 Mo3 3.2019(12) . ?
Mo1 Mo5 3.2820(11) . ?
Mo1 Mo6 3.4010(12) . ?
Mo1 O1 1.926(6) . ?
Mo1 O4 2.175(6) . ?
Mo1 O7 1.966(6) . ?
Mo1 O9 2.267(6) . ?
Mo1 O11 1.715(6) . ?
Mo1 O18 1.706(7) . ?
Mo2 Mo3 3.1702(13) . ?
Mo2 Mo4 3.2566(11) . ?
Mo2 Mo6 3.4337(11) . ?
Mo2 O4 2.155(6) . ?
Mo2 O5 2.266(6) . ?
Mo2 O6 1.983(6) . ?
Mo2 O10 1.920(6) . ?
Mo2 O12 1.741(6) . ?
Mo2 O25 1.695(7) . ?
Mo3 Mo6 3.4038(11) . ?
Mo3 O4 2.141(6) . ?
Mo3 O6 1.919(6) . ?
Mo3 O7 1.901(6) . ?
Mo3 O13 1.722(7) . ?
Mo3 O14 2.560(7) . ?
Mo3 O17 1.726(7) . ?
Mo4 Mo6 3.3983(12) . ?
Mo4 Mo8 3.2184(11) . ?
Mo4 O2 2.216(6) . ?
Mo4 O5 2.175(6) . ?
Mo4 O10 1.963(6) . ?
Mo4 O15 1.734(7) . ?
Mo4 O16 1.960(6) . ?
Mo4 O21 1.702(7) . ?
Mo5 Mo6 3.4083(12) . ?
Mo5 Mo8 3.1843(12) . ?
Mo5 O1 1.938(6) . ?
Mo5 O2 2.162(6) . ?
Mo5 O3 1.973(6) . ?
Mo5 O9 2.285(6) . ?
Mo5 O19 1.720(7) . ?
Mo5 O24 1.707(7) . ?
Mo6 Mo8 3.4130(12) . ?
Mo6 O2 2.289(6) . ?
Mo6 O4 2.250(6) . ?
Mo6 O5 1.913(6) . ?
Mo6 O8 1.738(6) . ?
Mo6 O9 1.870(6) . ?
Mo6 O14 1.738(6) . ?
Pd2 O8W 2.016(9) . ?
Pd2 O7W 2.075(9) . ?
Pd2 O6W 2.060(9) . ?
Pd2 O4W 2.034(9) . ?
Mo8 O2 2.123(6) . ?
Mo8 O3 1.925(6) . ?
Mo8 O8 2.480(7) . ?
Mo8 O16 1.939(6) . ?
Mo8 O23 1.720(7) . ?
Mo8 O26 1.714(7) . ?
Pd1 O5W 2.035(8) . ?
Pd1 O3W 2.025(9) . ?
Pd1 O2W 2.042(9) . ?
Pd1 O1W 2.029(9) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Mo5 Mo1 Mo3 123.17(3) . . ?
Mo6 Mo1 Mo3 61.97(2) . . ?
Mo6 Mo1 Mo5 61.30(2) . . ?
O1 Mo1 Mo3 131.91(19) . . ?
O1 Mo1 Mo5 31.96(18) . . ?
O1 Mo1 Mo6 80.39(19) . . ?
O4 Mo1 Mo3 41.70(16) . . ?
O4 Mo1 Mo5 89.73(15) . . ?
O4 Mo1 Mo6 40.58(15) . . ?
O4 Mo1 O1 90.2(2) . . ?
O7 Mo1 Mo3 33.44(17) . . ?
O7 Mo1 Mo5 127.26(19) . . ?
O7 Mo1 Mo6 74.59(19) . . ?
O7 Mo1 O1 154.8(3) . . ?
O7 Mo1 O4 72.4(2) . . ?
O9 Mo1 Mo3 85.82(15) . . ?
O9 Mo1 Mo5 44.07(16) . . ?
O9 Mo1 Mo6 31.06(14) . . ?
O9 Mo1 O1 73.9(2) . . ?
O9 Mo1 O4 71.6(2) . . ?
O9 Mo1 O7 83.3(2) . . ?
O11 Mo1 Mo3 126.5(2) . . ?
O11 Mo1 Mo5 87.0(2) . . ?
O11 Mo1 Mo6 121.7(2) . . ?
O11 Mo1 O1 97.8(3) . . ?
O11 Mo1 O4 158.9(3) . . ?
O11 Mo1 O7 93.2(3) . . ?
O11 Mo1 O9 91.9(3) . . ?
O18 Mo1 Mo3 88.5(2) . . ?
O18 Mo1 Mo5 130.7(2) . . ?
O18 Mo1 Mo6 134.1(2) . . ?
O18 Mo1 O1 98.8(3) . . ?
O18 Mo1 O4 93.9(3) . . ?
O18 Mo1 O7 100.4(3) . . ?
O18 Mo1 O9 163.4(3) . . ?
O18 Mo1 O11 104.0(3) . . ?
Mo4 Mo2 Mo3 122.43(3) . . ?
Mo6 Mo2 Mo3 61.90(2) . . ?
Mo6 Mo2 Mo4 60.99(2) . . ?
O4 Mo2 Mo3 42.28(16) . . ?
O4 Mo2 Mo4 86.81(15) . . ?
O4 Mo2 Mo6 39.78(16) . . ?
O5 Mo2 Mo3 88.42(16) . . ?
O5 Mo2 Mo4 41.76(16) . . ?
O5 Mo2 Mo6 31.52(15) . . ?
O5 Mo2 O4 70.8(2) . . ?
O6 Mo2 Mo3 35.00(18) . . ?
O6 Mo2 Mo4 126.83(18) . . ?
O6 Mo2 Mo6 73.46(17) . . ?
O6 Mo2 O4 73.5(2) . . ?
O6 Mo2 O5 85.1(2) . . ?
O10 Mo2 Mo3 129.37(19) . . ?
O10 Mo2 Mo4 33.41(19) . . ?
O10 Mo2 Mo6 81.20(19) . . ?
O10 Mo2 O4 87.2(2) . . ?
O10 Mo2 O5 73.0(2) . . ?
O10 Mo2 O6 154.7(3) . . ?
O12 Mo2 Mo3 128.6(2) . . ?
O12 Mo2 Mo4 88.0(2) . . ?
O12 Mo2 Mo6 121.3(2) . . ?
O12 Mo2 O4 159.1(3) . . ?
O12 Mo2 O5 92.0(3) . . ?
O12 Mo2 O6 93.8(3) . . ?
O12 Mo2 O10 99.4(3) . . ?
O25 Mo2 Mo3 87.1(2) . . ?
O25 Mo2 Mo4 130.2(2) . . ?
O25 Mo2 Mo6 134.2(2) . . ?
O25 Mo2 O4 94.6(3) . . ?
O25 Mo2 O5 162.2(3) . . ?
O25 Mo2 O6 100.8(3) . . ?
O25 Mo2 O10 96.8(3) . . ?
O25 Mo2 O12 104.2(3) . . ?
Mo2 Mo3 Mo1 82.50(3) . . ?
Mo6 Mo3 Mo1 61.89(2) . . ?
Mo6 Mo3 Mo2 62.86(2) . . ?
O4 Mo3 Mo1 42.51(16) . . ?
O4 Mo3 Mo2 42.62(15) . . ?
O4 Mo3 Mo6 40.34(16) . . ?
O6 Mo3 Mo1 117.31(19) . . ?
O6 Mo3 Mo2 36.34(19) . . ?
O6 Mo3 Mo6 74.81(18) . . ?
O6 Mo3 O4 75.0(2) . . ?
O7 Mo3 Mo1 34.75(19) . . ?
O7 Mo3 Mo2 116.49(19) . . ?
O7 Mo3 Mo6 75.13(19) . . ?
O7 Mo3 O4 74.4(2) . . ?
O7 Mo3 O6 147.6(3) . . ?
O13 Mo3 Mo1 93.5(2) . . ?
O13 Mo3 Mo2 91.9(2) . . ?
O13 Mo3 Mo6 145.5(2) . . ?
O13 Mo3 O4 105.2(3) . . ?
O13 Mo3 O6 99.2(3) . . ?
O13 Mo3 O7 98.7(3) . . ?
O14 Mo3 Mo1 84.92(14) . . ?
O14 Mo3 Mo2 82.54(15) . . ?
O14 Mo3 Mo6 29.83(14) . . ?
O14 Mo3 O4 70.1(2) . . ?
O14 Mo3 O6 76.8(2) . . ?
O14 Mo3 O7 83.0(2) . . ?
O14 Mo3 O13 174.4(3) . . ?
O17 Mo3 Mo1 132.3(2) . . ?
O17 Mo3 Mo2 137.5(2) . . ?
O17 Mo3 Mo6 107.9(2) . . ?
O17 Mo3 O4 148.2(3) . . ?
O17 Mo3 O6 101.9(3) . . ?
O17 Mo3 O7 98.5(3) . . ?
O17 Mo3 O13 106.5(3) . . ?
O17 Mo3 O14 78.4(3) . . ?
Mo6 Mo4 Mo2 62.08(2) . . ?
Mo8 Mo4 Mo2 123.83(3) . . ?
Mo8 Mo4 Mo6 62.03(2) . . ?
O2 Mo4 Mo2 90.61(15) . . ?
O2 Mo4 Mo6 41.85(16) . . ?
O2 Mo4 Mo8 41.01(15) . . ?
O5 Mo4 Mo2 43.94(15) . . ?
O5 Mo4 Mo6 31.38(14) . . ?
O5 Mo4 Mo8 87.24(15) . . ?
O5 Mo4 O2 73.1(2) . . ?
O10 Mo4 Mo2 32.58(18) . . ?
O10 Mo4 Mo6 81.62(19) . . ?
O10 Mo4 Mo8 131.32(19) . . ?
O10 Mo4 O2 90.3(2) . . ?
O10 Mo4 O5 74.3(2) . . ?
O15 Mo4 Mo2 125.2(2) . . ?
O15 Mo4 Mo6 131.7(2) . . ?
O15 Mo4 Mo8 89.2(2) . . ?
O15 Mo4 O2 90.6(3) . . ?
O15 Mo4 O5 158.8(3) . . ?
O15 Mo4 O10 92.7(3) . . ?
O16 Mo4 Mo2 131.2(2) . . ?
O16 Mo4 Mo6 76.9(2) . . ?
O16 Mo4 Mo8 34.14(19) . . ?
O16 Mo4 O2 73.3(2) . . ?
O16 Mo4 O5 87.3(2) . . ?
O16 Mo4 O10 158.5(3) . . ?
O16 Mo4 O15 101.2(3) . . ?
O21 Mo4 Mo2 86.8(2) . . ?
O21 Mo4 Mo6 122.5(3) . . ?
O21 Mo4 Mo8 128.9(3) . . ?
O21 Mo4 O2 161.5(3) . . ?
O21 Mo4 O5 92.6(3) . . ?
O21 Mo4 O10 97.1(3) . . ?
O21 Mo4 O15 105.8(3) . . ?
O21 Mo4 O16 94.8(3) . . ?
Mo6 Mo5 Mo1 61.07(2) . . ?
Mo8 Mo5 Mo1 122.41(3) . . ?
Mo8 Mo5 Mo6 62.25(2) . . ?
O1 Mo5 Mo1 31.74(19) . . ?
O1 Mo5 Mo6 80.05(18) . . ?
O1 Mo5 Mo8 127.44(19) . . ?
O2 Mo5 Mo1 86.98(15) . . ?
O2 Mo5 Mo6 41.42(16) . . ?
O2 Mo5 Mo8 41.52(15) . . ?
O2 Mo5 O1 85.9(2) . . ?
O3 Mo5 Mo1 130.07(19) . . ?
O3 Mo5 Mo6 74.85(18) . . ?
O3 Mo5 Mo8 34.72(18) . . ?
O3 Mo5 O1 154.7(3) . . ?
O3 Mo5 O2 73.4(2) . . ?
O9 Mo5 Mo1 43.63(15) . . ?
O9 Mo5 Mo6 31.08(15) . . ?
O9 Mo5 Mo8 88.29(16) . . ?
O9 Mo5 O1 73.2(2) . . ?
O9 Mo5 O2 72.1(2) . . ?
O9 Mo5 O3 86.5(2) . . ?
O19 Mo5 Mo1 84.9(2) . . ?
O19 Mo5 Mo6 115.3(2) . . ?
O19 Mo5 Mo8 129.1(2) . . ?
O19 Mo5 O1 98.9(3) . . ?
O19 Mo5 O2 155.3(3) . . ?
O19 Mo5 O3 94.4(3) . . ?
O19 Mo5 O9 86.0(3) . . ?
O24 Mo5 Mo1 128.4(2) . . ?
O24 Mo5 Mo6 139.4(3) . . ?
O24 Mo5 Mo8 90.3(3) . . ?
O24 Mo5 O1 97.1(3) . . ?
O24 Mo5 O2 98.1(3) . . ?
O24 Mo5 O3 100.0(3) . . ?
O24 Mo5 O9 166.4(3) . . ?
O24 Mo5 O19 105.3(3) . . ?
Mo2 Mo6 Mo1 75.86(2) . . ?
Mo3 Mo6 Mo1 56.14(2) . . ?
Mo3 Mo6 Mo2 55.24(2) . . ?
Mo4 Mo6 Mo1 101.47(3) . . ?
Mo4 Mo6 Mo2 56.93(2) . . ?
Mo4 Mo6 Mo3 111.81(3) . . ?
Mo5 Mo6 Mo1 57.63(2) . . ?
Mo5 Mo6 Mo2 105.44(3) . . ?
Mo5 Mo6 Mo3 113.68(3) . . ?
Mo5 Mo6 Mo4 78.02(3) . . ?
Mo8 Mo6 Mo1 112.54(3) . . ?
Mo8 Mo6 Mo2 113.10(3) . . ?
Mo8 Mo6 Mo3 163.84(3) . . ?
Mo8 Mo6 Mo4 56.39(2) . . ?
Mo8 Mo6 Mo5 55.66(2) . . ?
O2 Mo6 Mo1 82.22(15) . . ?
O2 Mo6 Mo2 85.04(15) . . ?
O2 Mo6 Mo3 126.29(15) . . ?
O2 Mo6 Mo4 40.22(15) . . ?
O2 Mo6 Mo5 38.68(15) . . ?
O2 Mo6 Mo8 37.58(15) . . ?
O4 Mo6 Mo1 38.96(15) . . ?
O4 Mo6 Mo2 37.80(15) . . ?
O4 Mo6 Mo3 38.04(16) . . ?
O4 Mo6 Mo4 81.95(15) . . ?
O4 Mo6 Mo5 85.34(15) . . ?
O4 Mo6 Mo8 125.80(16) . . ?
O4 Mo6 O2 88.3(2) . . ?
O5 Mo6 Mo1 111.28(19) . . ?
O5 Mo6 Mo2 38.27(18) . . ?
O5 Mo6 Mo3 88.00(17) . . ?
O5 Mo6 Mo4 36.30(18) . . ?
O5 Mo6 Mo5 112.82(18) . . ?
O5 Mo6 Mo8 86.08(17) . . ?
O5 Mo6 O2 76.4(2) . . ?
O5 Mo6 O4 75.6(2) . . ?
O8 Mo6 Mo1 141.2(2) . . ?
O8 Mo6 Mo2 137.0(2) . . ?
O8 Mo6 Mo3 152.0(2) . . ?
O8 Mo6 Mo4 88.3(2) . . ?
O8 Mo6 Mo5 88.8(2) . . ?
O8 Mo6 Mo8 44.1(2) . . ?
O8 Mo6 O2 81.7(3) . . ?
O8 Mo6 O4 169.5(3) . . ?
O8 Mo6 O5 98.8(3) . . ?
O9 Mo6 Mo1 38.71(18) . . ?
O9 Mo6 Mo2 113.48(18) . . ?
O9 Mo6 Mo3 86.61(18) . . ?
O9 Mo6 Mo4 114.4(2) . . ?
O9 Mo6 Mo5 39.09(19) . . ?
O9 Mo6 Mo8 89.01(18) . . ?
O9 Mo6 O2 77.4(3) . . ?
O9 Mo6 O4 77.6(2) . . ?
O9 Mo6 O5 142.7(3) . . ?
O9 Mo6 O8 103.1(3) . . ?
O14 Mo6 Mo1 93.7(2) . . ?
O14 Mo6 Mo2 88.5(2) . . ?
O14 Mo6 Mo3 47.1(2) . . ?
O14 Mo6 Mo4 136.3(2) . . ?
O14 Mo6 Mo5 142.1(2) . . ?
O14 Mo6 Mo8 148.9(2) . . ?
O14 Mo6 O2 173.0(3) . . ?
O14 Mo6 O4 85.0(3) . . ?
O14 Mo6 O5 100.0(3) . . ?
O14 Mo6 O8 104.9(3) . . ?
O14 Mo6 O9 103.0(3) . . ?
O7W Pd2 O8W 87.9(4) . . ?
O6W Pd2 O8W 88.5(4) . . ?
O6W Pd2 O7W 176.3(4) . . ?
O4W Pd2 O8W 179.6(3) . . ?
O4W Pd2 O7W 92.1(4) . . ?
O4W Pd2 O6W 91.5(4) . . ?
Mo5 Mo8 Mo4 84.00(3) . . ?
Mo6 Mo8 Mo4 61.57(2) . . ?
Mo6 Mo8 Mo5 62.10(2) . . ?
O2 Mo8 Mo4 43.23(16) . . ?
O2 Mo8 Mo5 42.48(16) . . ?
O2 Mo8 Mo6 41.12(17) . . ?
O3 Mo8 Mo4 118.39(17) . . ?
O3 Mo8 Mo5 35.71(18) . . ?
O3 Mo8 Mo6 75.19(18) . . ?
O3 Mo8 O2 75.2(2) . . ?
O8 Mo8 Mo4 81.73(15) . . ?
O8 Mo8 Mo5 83.09(15) . . ?
O8 Mo8 Mo6 29.20(14) . . ?
O8 Mo8 O2 70.3(2) . . ?
O8 Mo8 O3 80.0(2) . . ?
O16 Mo8 Mo4 34.56(19) . . ?
O16 Mo8 Mo5 118.04(19) . . ?
O16 Mo8 Mo6 76.68(19) . . ?
O16 Mo8 O2 75.9(2) . . ?
O16 Mo8 O3 149.5(2) . . ?
O16 Mo8 O8 81.2(3) . . ?
O23 Mo8 Mo4 133.5(2) . . ?
O23 Mo8 Mo5 134.1(2) . . ?
O23 Mo8 Mo6 108.1(3) . . ?
O23 Mo8 O2 149.3(3) . . ?
O23 Mo8 O3 99.3(3) . . ?
O23 Mo8 O8 79.0(3) . . ?
O23 Mo8 O16 100.5(3) . . ?
O26 Mo8 Mo4 96.6(2) . . ?
O26 Mo8 Mo5 93.0(3) . . ?
O26 Mo8 Mo6 147.0(3) . . ?
O26 Mo8 O2 105.9(3) . . ?
O26 Mo8 O3 97.6(3) . . ?
O26 Mo8 O8 175.9(3) . . ?
O26 Mo8 O16 99.5(3) . . ?
O26 Mo8 O23 104.8(4) . . ?
O3W Pd1 O5W 91.2(4) . . ?
O2W Pd1 O5W 175.8(4) . . ?
O2W Pd1 O3W 89.5(4) . . ?
O1W Pd1 O5W 90.1(4) . . ?
O1W Pd1 O3W 178.6(4) . . ?
O1W Pd1 O2W 89.2(4) . . ?
Mo5 O1 Mo1 116.3(3) . . ?
Mo5 O2 Mo4 156.2(3) . . ?
Mo6 O2 Mo4 97.9(2) . . ?
Mo6 O2 Mo5 99.9(2) . . ?
Mo8 O2 Mo4 95.8(2) . . ?
Mo8 O2 Mo5 96.0(2) . . ?
Mo8 O2 Mo6 101.3(3) . . ?
Mo8 O3 Mo5 109.6(3) . . ?
Mo2 O4 Mo1 152.0(3) . . ?
Mo3 O4 Mo1 95.8(2) . . ?
Mo3 O4 Mo2 95.1(2) . . ?
Mo6 O4 Mo1 100.5(2) . . ?
Mo6 O4 Mo2 102.4(2) . . ?
Mo6 O4 Mo3 101.6(3) . . ?
Mo4 O5 Mo2 94.3(2) . . ?
Mo6 O5 Mo2 110.2(3) . . ?
Mo6 O5 Mo4 112.3(3) . . ?
Mo3 O6 Mo2 108.7(3) . . ?
Mo3 O7 Mo1 111.8(3) . . ?
Mo8 O8 Mo6 106.7(3) . . ?
Mo5 O9 Mo1 92.3(2) . . ?
Mo6 O9 Mo1 110.2(3) . . ?
Mo6 O9 Mo5 109.8(3) . . ?
Mo4 O10 Mo2 114.0(3) . . ?
Mo6 O14 Mo3 103.1(3) . . ?
Mo8 O16 Mo4 111.3(3) . . ?

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_compound4
_database_code_depnum_ccdc_archive 'CCDC 2042537'
loop_
_audit_author_name
_audit_author_address
'Hai Fu'
;CCUT china
China
;
_audit_update_record             
;
2020-11-05 deposited with the CCDC.	2021-01-07 downloaded from the CCDC.
;
_audit_creation_date             2020-11-04
_audit_creation_method           
;
Olex2 1.2
(compiled 2014.09.19 svn.r3010 for OlexSys, GUI svn.r4874)
;
_chemical_formula_moiety         'Mo4 O17 Pd, H8 O4 Pd, 2(H2 O)'
_chemical_formula_sum            'H12 Mo4 O23 Pd2'
_chemical_formula_weight         976.64
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_Cromer_Mann_a1
_atom_type_scat_Cromer_Mann_a2
_atom_type_scat_Cromer_Mann_a3
_atom_type_scat_Cromer_Mann_a4
_atom_type_scat_Cromer_Mann_b1
_atom_type_scat_Cromer_Mann_b2
_atom_type_scat_Cromer_Mann_b3
_atom_type_scat_Cromer_Mann_b4
_atom_type_scat_Cromer_Mann_c
_atom_type_scat_source
_atom_type_scat_dispersion_source
H 0.00000 0.00000 0.49300 0.32291 0.14019 0.04081 10.51090 26.12570 3.14236
57.79970 0.0030380000826
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)' custom
Mo -1.68300 0.68600 3.70300 17.23600 12.88800 3.74300 0.27700 1.09600 11.00400
61.65800 4.388 'Custom 4-Gaussian' custom
O 0.01100 0.00600 3.04900 2.28700 1.54600 0.86700 13.27700 5.70100 0.32400
32.90900 0.251 'Custom 4-Gaussian' custom
Pd -0.99900 1.00700 19.33200 15.50200 5.29500 0.60600 0.69900 7.98900 25.20500
76.89900 5.266 'Custom 4-Gaussian' custom

_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,-y,-z

_symmetry_Int_Tables_number      2
_cell_length_a                   10.0495(10)
_cell_length_b                   10.1019(10)
_cell_length_c                   10.4574(10)
_cell_angle_alpha                69.406(2)
_cell_angle_beta                 84.106(2)
_cell_angle_gamma                88.251(1)
_cell_volume                     988.51(17)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    9957
_cell_measurement_theta_max      28.323
_cell_measurement_theta_min      2.957
_exptl_absorpt_coefficient_mu    4.345
_exptl_absorpt_correction_type   none
_exptl_crystal_density_diffrn    3.2811
_exptl_crystal_F_000             894.7665
_diffrn_reflns_av_R_equivalents  0.0461
_diffrn_reflns_av_unetI/netI     0.0313
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            14520
_diffrn_reflns_theta_full        28.3220
_diffrn_reflns_theta_max         28.32
_diffrn_reflns_theta_min         2.77
_diffrn_measured_fraction_theta_full 0.9986
_diffrn_measured_fraction_theta_max 0.9974
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_reflns_Friedel_coverage         0.0
_reflns_limit_h_max              13
_reflns_limit_h_min              -13
_reflns_limit_k_max              13
_reflns_limit_k_min              -12
_reflns_limit_l_max              13
_reflns_limit_l_min              0
_reflns_number_gt                4653
_reflns_number_total             4916
_reflns_threshold_expression     I>=2u(I)
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'olex2.refine (Bourhis et al., 2013)'
_refine_diff_density_max         1.6518
_refine_diff_density_min         -2.8426
_refine_diff_density_rms         0.3481
_refine_ls_d_res_high            0.7490
_refine_ls_d_res_low             7.3469
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_goodness_of_fit_ref   1.0232
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_constraints    18
_refine_ls_number_parameters     247
_refine_ls_number_reflns         4916
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0370
_refine_ls_R_factor_gt           0.0341
_refine_ls_restrained_S_all      1.0232
_refine_ls_shift/su_max          0.0020
_refine_ls_shift/su_mean         0.0002
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0644P)²+10.6391P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1016
_refine_ls_wR_factor_ref         0.1111
_olex2_refinement_description    
;
1. Fixed Uiso
 At 1.5 times of:
  All O(H,H) groups
2.a Free rotating group:
 O15W(H15a,H15b), O17W(H17a,H17b)
2.b Rotating group:
 O7W(H7Wa,H7Wb), O8W(H8Wa,H8Wb), O9W(H9Wa,H9Wb), O10W(H10a,H10b)
;
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_refinement_flags_posn
Pd3 Pd 0.469790(4) 0.762003(4) 0.171900(4) 0.02023(9) Uani 1.000000 .
Mo1 Mo 0.167143(4) 0.538350(4) 0.454382(4) 0.00890(8) Uani 1.000000 .
Mo3 Mo 0.043318(4) 0.204163(4) 0.639027(4) 0.01138(9) Uani 1.000000 .
Mo6 Mo 0.082271(4) 0.293666(4) 0.307841(4) 0.01145(9) Uani 1.000000 .
Mo8 Mo 0.156141(4) 0.624015(4) 0.117930(4) 0.01175(9) Uani 1.000000 .
O1 O -0.014521(4) 0.385900(4) 0.461760(4) 0.0110(2) Uani 1.000000 .
O1W O 0.524713(4) 0.594620(4) 0.266839(4) 0.027622(4) Uiso 1.000000 .
O2 O 0.066429(4) 0.672758(4) 0.289267(4) 0.0115(2) Uani 1.000000 .
O2W O 0.573386(4) 0.817942(4) 0.018045(4) 0.031219(4) Uiso 1.000000 .
O3 O 0.031575(4) 0.471895(4) 0.170193(4) 0.0147(2) Uani 1.000000 .
O3W O 0.491049(4) 0.879359(4) 0.256140(4) 0.024788(4) Uiso 1.000000 .
O4 O 0.153189(4) 0.189999(4) 0.481973(4) 0.0141(2) Uani 1.000000 .
O5 O 0.223438(4) 0.469581(4) 0.310736(4) 0.0113(2) Uani 1.000000 .
O9 O 0.291427(4) 0.652557(4) 0.445421(4) 0.0204(2) Uani 1.000000 .
O11 O 0.194952(4) 0.388577(4) 0.597555(4) 0.0144(2) Uani 1.000000 .
O12 O -0.059619(4) 0.202659(4) 0.317689(4) 0.0223(2) Uani 1.000000 .
O13 O 0.197549(4) 0.240522(4) 0.202940(4) 0.0212(2) Uani 1.000000 .
O15 O 0.064586(4) 0.752240(4) 0.009273(4) 0.0217(2) Uani 1.000000 .
O20 O 0.295013(4) 0.760209(4) 0.131458(4) 0.0190(2) Uani 1.000000 .
O23 O -0.079671(4) 0.088844(4) 0.647508(4) 0.0235(2) Uani 1.000000 .
O25 O 0.272396(4) 0.567984(4) 0.013866(4) 0.0245(2) Uani 1.000000 .
O26 O 0.129867(4) 0.117776(4) 0.779543(4) 0.0242(2) Uani 1.000000 .
Pd1 Pd 0.571803(4) 0.202472(4) 0.340055(4) 0.01324(8) Uani 1.000000 .
O7W O 0.478637(4) 0.332862(4) 0.177933(4) 0.0351(2) Uani 1.000000 .
H7Wa H 0.441313(4) 0.283572(4) 0.140344(4) 0.0527(3) Uiso 1.000000 GR
H7Wb H 0.537074(4) 0.381823(4) 0.116094(4) 0.0527(3) Uiso 1.000000 GR
O8W O 0.671539(4) 0.079355(4) 0.503378(4) 0.0334(2) Uani 1.000000 .
H8Wa H 0.736067(4) 0.126489(4) 0.512876(4) 0.0500(3) Uiso 1.000000 GR
H8Wb H 0.708811(4) 0.011032(4) 0.484262(4) 0.0500(3) Uiso 1.000000 GR
O9W O 0.679510(4) 0.115154(4) 0.213601(4) 0.0368(2) Uani 1.000000 .
H9Wa H 0.761947(4) 0.115745(4) 0.225220(4) 0.0552(3) Uiso 1.000000 GR
H9Wb H 0.659484(4) 0.028026(4) 0.238122(4) 0.0552(3) Uiso 1.000000 GR
O10W O 0.460067(4) 0.293829(4) 0.460007(4) 0.0331(2) Uani 1.000000 .
H10a H 0.500336(4) 0.286450(4) 0.529792(4) 0.0496(3) Uiso 1.000000 GR
H10b H 0.455958(4) 0.382370(4) 0.416995(4) 0.0496(3) Uiso 1.000000 GR
O15W O 0.179168(4) 0.035614(4) 0.066858(4) 0.040179(4) Uiso 1.000000 .
H15a H 0.253471(4) 0.079394(4) 0.049890(4) 0.060269(5) Uiso 1.000000 G
H15b H 0.200525(4) -0.049732(4) 0.079086(4) 0.060269(5) Uiso 1.000000 G
O17W O 0.790513(4) 0.603257(4) 0.133690(4) 0.050841(4) Uiso 1.000000 .
H17a H 0.839494(4) 0.530513(4) 0.160734(4) 0.076262(5) Uiso 1.000000 G
H17b H 0.733347(4) 0.594921(4) 0.201905(4) 0.076262(5) Uiso 1.000000 G


loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Pd3 O1W 1.73897(14) . ?
Pd3 O2W 1.74474(14) . ?
Pd3 O3W 1.73666(14) . ?
Pd3 O20 1.85043(18) . ?
Mo1 Mo1 3.4317(3) 2_566 ?
Mo1 Mo3 3.2395(2) 2_566 ?
Mo1 Mo3 3.4425(3) . ?
Mo1 Mo6 3.4996(2) . ?
Mo1 Mo8 3.3275(3) . ?
Mo1 O1 2.40201(18) . ?
Mo1 O1 1.95735(14) 2_566 ?
Mo1 O2 2.11545(14) . ?
Mo1 O5 1.89599(15) . ?
Mo1 O9 1.69932(13) . ?
Mo1 O11 1.75369(13) . ?
Mo3 Mo6 3.2413(3) . ?
Mo3 O1 2.21511(16) . ?
Mo3 O2 1.93051(13) 2_566 ?
Mo3 O4 1.92880(15) . ?
Mo3 O11 2.33449(18) . ?
Mo3 O23 1.69862(13) . ?
Mo3 O26 1.72955(13) . ?
Mo6 Mo8 3.2891(3) . ?
Mo6 O1 2.25462(16) . ?
Mo6 O3 1.96077(15) . ?
Mo6 O4 1.94935(15) . ?
Mo6 O5 2.31777(18) . ?
Mo6 O12 1.69478(14) . ?
Mo6 O13 1.71727(12) . ?
Mo8 O2 2.12777(17) . ?
Mo8 O3 1.90087(15) . ?
Mo8 O5 2.22695(16) . ?
Mo8 O15 1.70940(11) . ?
Mo8 O20 2.03844(15) . ?
Mo8 O25 1.73246(12) . ?
Pd1 O7W 2.04099(14) . ?
Pd1 O8W 2.06146(14) . ?
Pd1 O9W 2.04124(14) . ?
Pd1 O10W 2.03665(13) . ?
O7W H7Wa 0.8500 . ?
O7W H7Wb 0.8500 . ?
O8W H8Wa 0.8500 . ?
O8W H8Wb 0.8500 . ?
O9W H9Wa 0.8501 . ?
O9W H9Wb 0.8499 . ?
O10W H10a 0.8500 . ?
O10W H10b 0.8500 . ?
O15W H15a 0.8499 . ?
O15W H15b 0.8500 . ?
O17W H17a 0.8500 . ?
O17W H17b 0.8500 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2W Pd3 O1W 106.333(3) . . ?
O3W Pd3 O1W 110.170(3) . . ?
O3W Pd3 O2W 107.687(3) . . ?
O20 Pd3 O1W 112.399(2) . . ?
O20 Pd3 O2W 108.382(3) . . ?
O20 Pd3 O3W 111.602(3) . . ?
Mo6 Mo1 Mo3 55.6588(10) . . ?
Mo6 Mo1 Mo3 106.2427(14) . 2_566 ?
Mo8 Mo1 Mo3 112.6193(15) . . ?
Mo8 Mo1 Mo3 73.1988(12) . 2_566 ?
Mo8 Mo1 Mo6 57.5346(11) . . ?
O1 Mo1 Mo3 39.7565(11) . . ?
O1 Mo1 Mo3 88.2161(15) 2_566 . ?
O1 Mo1 Mo3 86.3107(15) . 2_566 ?
O1 Mo1 Mo3 42.0369(13) 2_566 2_566 ?
O1 Mo1 Mo6 39.7087(13) . . ?
O1 Mo1 Mo6 114.509(2) 2_566 . ?
O1 Mo1 Mo8 81.7800(15) . . ?
O1 Mo1 Mo8 111.9311(18) 2_566 . ?
O2 Mo1 Mo3 119.7450(19) . . ?
O2 Mo1 Mo3 34.8881(14) . 2_566 ?
O2 Mo1 Mo6 80.0907(18) . . ?
O2 Mo1 Mo8 38.4852(14) . . ?
O2 Mo1 O1 79.9892(18) . . ?
O2 Mo1 O1 74.2366(19) . 2_566 ?
O5 Mo1 Mo3 87.1471(17) . . ?
O5 Mo1 Mo3 112.1181(19) . 2_566 ?
O5 Mo1 Mo6 37.9103(14) . . ?
O5 Mo1 Mo8 39.7020(13) . . ?
O5 Mo1 O1 77.133(2) . . ?
O5 Mo1 O1 143.989(3) . 2_566 ?
O5 Mo1 O2 77.280(2) . . ?
O9 Mo1 Mo3 142.612(2) . . ?
O9 Mo1 Mo3 91.1615(19) . 2_566 ?
O9 Mo1 Mo6 141.073(2) . . ?
O9 Mo1 Mo8 96.9826(18) . . ?
O9 Mo1 O1 101.832(3) . 2_566 ?
O9 Mo1 O1 177.416(2) . . ?
O9 Mo1 O2 97.624(2) . . ?
O9 Mo1 O5 103.378(2) . . ?
O11 Mo1 Mo3 38.2929(17) . . ?
O11 Mo1 Mo3 139.699(2) . 2_566 ?
O11 Mo1 Mo6 84.727(2) . . ?
O11 Mo1 Mo8 138.720(2) . . ?
O11 Mo1 O1 77.9977(19) . . ?
O11 Mo1 O1 97.877(2) . 2_566 ?
O11 Mo1 O2 157.817(3) . . ?
O11 Mo1 O5 100.300(2) . . ?
O11 Mo1 O9 104.335(3) . . ?
Mo6 Mo3 Mo1 63.0634(11) . . ?
Mo6 Mo3 Mo1 78.3896(12) . 2_566 ?
O1 Mo3 Mo1 43.9067(13) . . ?
O1 Mo3 Mo1 36.2770(13) . 2_566 ?
O1 Mo3 Mo6 44.0010(14) . . ?
O2 Mo3 Mo1 75.4365(15) 2_566 . ?
O2 Mo3 Mo1 38.8123(14) 2_566 2_566 ?
O2 Mo3 Mo6 116.3157(17) 2_566 . ?
O2 Mo3 O1 72.4636(18) 2_566 . ?
O4 Mo3 Mo1 73.4745(15) . . ?
O4 Mo3 Mo1 110.7507(17) . 2_566 ?
O4 Mo3 Mo6 33.5033(13) . . ?
O4 Mo3 O1 74.7326(18) . . ?
O4 Mo3 O2 145.413(2) . 2_566 ?
O11 Mo3 Mo1 27.7432(11) . . ?
O11 Mo3 Mo1 82.7719(15) . 2_566 ?
O11 Mo3 Mo6 83.3179(14) . . ?
O11 Mo3 O1 71.6065(16) . . ?
O11 Mo3 O2 80.116(2) . 2_566 ?
O11 Mo3 O4 79.4576(19) . . ?
O23 Mo3 Mo1 142.848(2) . . ?
O23 Mo3 Mo1 89.3695(19) . 2_566 ?
O23 Mo3 Mo6 90.019(2) . . ?
O23 Mo3 O1 98.967(2) . . ?
O23 Mo3 O2 97.009(2) . 2_566 ?
O23 Mo3 O4 98.610(3) . . ?
O23 Mo3 O11 170.569(2) . . ?
O26 Mo3 Mo1 138.274(3) . 2_566 ?
O26 Mo3 Mo1 112.638(2) . . ?
O26 Mo3 Mo6 139.205(2) . . ?
O26 Mo3 O1 156.105(3) . . ?
O26 Mo3 O2 99.778(3) . 2_566 ?
O26 Mo3 O4 105.853(2) . . ?
O26 Mo3 O11 84.907(2) . . ?
O26 Mo3 O23 104.468(2) . . ?
Mo3 Mo6 Mo1 61.2779(11) . . ?
Mo8 Mo6 Mo1 58.6039(11) . . ?
Mo8 Mo6 Mo3 119.2285(16) . . ?
O1 Mo6 Mo1 42.8946(13) . . ?
O1 Mo6 Mo3 43.0392(12) . . ?
O1 Mo6 Mo8 84.7985(15) . . ?
O3 Mo6 Mo1 78.8147(18) . . ?
O3 Mo6 Mo3 127.779(2) . . ?
O3 Mo6 Mo8 31.0576(14) . . ?
O3 Mo6 O1 84.868(2) . . ?
O4 Mo6 Mo1 71.8354(18) . . ?
O4 Mo6 Mo3 33.1043(14) . . ?
O4 Mo6 Mo8 124.926(2) . . ?
O4 Mo6 O1 73.4329(19) . . ?
O4 Mo6 O3 150.646(3) . . ?
O5 Mo6 Mo1 30.1731(12) . . ?
O5 Mo6 Mo3 85.8708(17) . . ?
O5 Mo6 Mo8 42.5572(12) . . ?
O5 Mo6 O1 72.6348(18) . . ?
O5 Mo6 O3 72.1682(18) . . ?
O5 Mo6 O4 82.457(2) . . ?
O12 Mo6 Mo1 133.513(2) . . ?
O12 Mo6 Mo3 88.6184(19) . . ?
O12 Mo6 Mo8 128.046(2) . . ?
O12 Mo6 O1 90.747(2) . . ?
O12 Mo6 O3 97.000(2) . . ?
O12 Mo6 O4 102.699(2) . . ?
O12 Mo6 O5 160.618(3) . . ?
O13 Mo6 Mo1 121.091(2) . . ?
O13 Mo6 Mo3 130.867(2) . . ?
O13 Mo6 Mo8 88.7792(17) . . ?
O13 Mo6 O1 163.189(3) . . ?
O13 Mo6 O3 97.551(2) . . ?
O13 Mo6 O4 97.931(2) . . ?
O13 Mo6 O5 92.186(2) . . ?
O13 Mo6 O12 105.388(3) . . ?
Mo6 Mo8 Mo1 63.8615(11) . . ?
O2 Mo8 Mo1 38.2219(13) . . ?
O2 Mo8 Mo6 85.2015(15) . . ?
O3 Mo8 Mo1 84.3019(17) . . ?
O3 Mo8 Mo6 32.1513(13) . . ?
O3 Mo8 O2 86.883(2) . . ?
O5 Mo8 Mo1 32.9467(14) . . ?
O5 Mo8 Mo6 44.7415(14) . . ?
O5 Mo8 O2 70.3739(17) . . ?
O5 Mo8 O3 75.3638(18) . . ?
O15 Mo8 Mo1 129.112(2) . . ?
O15 Mo8 Mo6 131.077(2) . . ?
O15 Mo8 O2 90.986(2) . . ?
O15 Mo8 O3 99.003(2) . . ?
O15 Mo8 O5 160.606(3) . . ?
O20 Mo8 Mo1 76.4024(17) . . ?
O20 Mo8 Mo6 131.5948(18) . . ?
O20 Mo8 O2 79.491(2) . . ?
O20 Mo8 O3 160.555(3) . . ?
O20 Mo8 O5 86.950(2) . . ?
O20 Mo8 O15 95.068(2) . . ?
O25 Mo8 Mo1 123.743(2) . . ?
O25 Mo8 Mo6 90.4279(18) . . ?
O25 Mo8 O2 160.658(3) . . ?
O25 Mo8 O3 99.363(3) . . ?
O25 Mo8 O5 93.362(2) . . ?
O25 Mo8 O15 105.926(3) . . ?
O25 Mo8 O20 89.531(2) . . ?
Mo3 O1 Mo1 101.686(2) . 2_566 ?
Mo3 O1 Mo1 96.3368(19) . . ?
Mo6 O1 Mo1 97.3966(18) . . ?
Mo6 O1 Mo1 152.930(3) . 2_566 ?
Mo6 O1 Mo3 92.9598(19) . . ?
Mo3 O2 Mo1 106.300(2) 2_566 . ?
Mo8 O2 Mo1 103.293(2) . . ?
Mo8 O2 Mo3 149.531(2) . 2_566 ?
Mo8 O3 Mo6 116.791(2) . . ?
Mo6 O4 Mo3 113.392(2) . . ?
Mo6 O5 Mo1 111.917(2) . . ?
Mo8 O5 Mo1 107.351(2) . . ?
Mo8 O5 Mo6 92.701(2) . . ?
Mo3 O11 Mo1 113.964(2) . . ?
Mo8 O20 Pd3 140.301(2) . . ?
O8W Pd1 O7W 177.123(3) . . ?
O9W Pd1 O7W 90.173(2) . . ?
O9W Pd1 O8W 90.576(2) . . ?
O10W Pd1 O7W 87.594(2) . . ?
O10W Pd1 O8W 91.668(2) . . ?
O10W Pd1 O9W 177.748(2) . . ?
H7Wa O7W Pd1 109.5 . . ?
H7Wb O7W Pd1 109.3 . . ?
H7Wb O7W H7Wa 104.5 . . ?
H8Wa O8W Pd1 109.5 . . ?
H8Wb O8W Pd1 109.2 . . ?
H8Wb O8W H8Wa 104.5 . . ?
H9Wa O9W Pd1 109.2 . . ?
H9Wb O9W Pd1 109.6 . . ?
H9Wb O9W H9Wa 104.5 . . ?
H10a O10W Pd1 109.5 . . ?
H10b O10W Pd1 109.3 . . ?
H10b O10W H10a 104.5 . . ?
H15b O15W H15a 104.5 . . ?
H17b O17W H17a 104.5 . . ?

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_compound3
_database_code_depnum_ccdc_archive 'CCDC 2042536'
loop_
_audit_author_name
_audit_author_address
'Hai Fu'
;CCUT china
China
;
_audit_update_record             
;
2020-11-05 deposited with the CCDC.	2021-01-07 downloaded from the CCDC.
;
_audit_creation_date             2020-11-04
_audit_creation_method           
;
Olex2 1.2
(compiled 2014.09.19 svn.r3010 for OlexSys, GUI svn.r4874)
;
_chemical_formula_moiety         'Mo4 O13.5, H8 O4 Pd, H2 O'
_chemical_formula_sum            'H10 Mo4 O18.5 Pd'
_chemical_formula_weight         796.21
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_Cromer_Mann_a1
_atom_type_scat_Cromer_Mann_a2
_atom_type_scat_Cromer_Mann_a3
_atom_type_scat_Cromer_Mann_a4
_atom_type_scat_Cromer_Mann_b1
_atom_type_scat_Cromer_Mann_b2
_atom_type_scat_Cromer_Mann_b3
_atom_type_scat_Cromer_Mann_b4
_atom_type_scat_Cromer_Mann_c
_atom_type_scat_source
_atom_type_scat_dispersion_source
H 0.00000 0.00000 0.49300 0.32291 0.14019 0.04081 10.51090 26.12570 3.14236
57.79970 0.0030380000826
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Mo -1.68402 0.70339 3.70250 17.23560 12.88760 3.74290 0.27720 1.09580 11.00400
61.65840 4.38749980927
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
O 0.01158 0.00611 3.04850 2.28680 1.54630 0.86700 13.27710 5.70110 0.32390
32.90890 0.250800013542
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Pd -0.98845 1.01473 19.33190 15.50170 5.29537 0.60584 0.69866 7.98929 25.20520
76.89860 5.26593017578
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'

_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_H-M_alt        'C 1 2/c 1'
_space_group_name_Hall           '-C 2yc'
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,y,-z+1/2
3 -x,-y,-z
4 x,-y,z-1/2
5 x+1/2,y+1/2,z
6 -x+1/2,y+1/2,-z+1/2
7 -x+1/2,-y+1/2,-z
8 x+1/2,-y+1/2,z-1/2

_symmetry_Int_Tables_number      15
_cell_length_a                   15.445(3)
_cell_length_b                   20.196(4)
_cell_length_c                   10.591(2)
_cell_angle_alpha                90
_cell_angle_beta                 91.985(2)
_cell_angle_gamma                90
_cell_volume                     3301.5(11)
_cell_formula_units_Z            8
_cell_measurement_reflns_used    9810
_cell_measurement_theta_max      28.372
_cell_measurement_theta_min      8.954
_exptl_absorpt_coefficient_mu    4.111
_exptl_absorpt_correction_type   none
_exptl_crystal_density_diffrn    3.2037
_exptl_crystal_F_000             2914.5966
_diffrn_reflns_av_R_equivalents  0.0483
_diffrn_reflns_av_unetI/netI     0.0256
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       -26
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            18995
_diffrn_reflns_theta_full        28.4266
_diffrn_reflns_theta_max         28.43
_diffrn_reflns_theta_min         8.94
_diffrn_ambient_temperature      0.0
_diffrn_measured_fraction_theta_full 0.9574
_diffrn_measured_fraction_theta_max 0.9553
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_reflns_Friedel_coverage         0.0
_reflns_limit_h_max              20
_reflns_limit_h_min              -20
_reflns_limit_k_max              26
_reflns_limit_k_min              0
_reflns_limit_l_max              14
_reflns_limit_l_min              0
_reflns_number_gt                3707
_reflns_number_total             3975
_reflns_threshold_expression     I>=2u(I)
_computing_cell_refinement       'SAINT v8.34A (Bruker, 2013)'
_computing_data_reduction        'SAINT v8.34A (Bruker, 2013)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'olex2.refine (Bourhis et al., 2013)'
_refine_diff_density_max         0.7204
_refine_diff_density_min         -0.8997
_refine_diff_density_rms         0.1573
_refine_ls_d_res_high            0.7465
_refine_ls_d_res_low             2.2877
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_goodness_of_fit_ref   1.0630
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_constraints    18
_refine_ls_number_parameters     224
_refine_ls_number_reflns         3975
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0259
_refine_ls_R_factor_gt           0.0231
_refine_ls_restrained_S_all      1.0630
_refine_ls_shift/su_max          0.0013
_refine_ls_shift/su_mean         0.0001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0281P)²+19.2045P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0589
_refine_ls_wR_factor_ref         0.0614
_olex2_refinement_description    
;
1. Fixed Uiso
 At 1.5 times of:
  All O(H,H) groups
2. Others
 Fixed Sof: H5Wa(0.5) H5Wb(0.5) H6Wa(0.5) H6Wb(0.5)
3.a Free rotating group:
 O5W(H5Wa,H5Wb), O6W(H6Wa,H6Wb)
3.b Rotating group:
 O4W(H4Wa,H4Wb), O3W(H3Wa,H3Wb), O2W(H2Wa,H2Wb), O1W(H1Wa,H1Wb)
;
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Mo1 Mo 0.218578(6) 0.233911(6) 0.655399(7) 0.01208(7) Uani 1.000000 1 . . .
Pd1 Pd 0.302247(6) 0.090208(6) 0.943058(7) 0.01781(7) Uani 1.000000 1 . . .
Mo3 Mo 0.358941(6) 0.135143(6) 0.483817(7) 0.01481(7) Uani 1.000000 1 . . .
Mo4 Mo 0.008260(6) 0.198835(6) 0.584617(7) 0.01521(7) Uani 1.000000 1 . . .
Mo5 Mo 0.151635(6) 0.103255(6) 0.457727(7) 0.01616(7) Uani 1.000000 1 . . .
O1 O 0.260258(7) 0.309820(7) 0.561417(7) 0.0150(4) Uani 1.000000 1 . . .
O2 O 0.139611(7) 0.163009(7) 0.640793(7) 0.0150(4) Uani 1.000000 1 . . .
O3 O 0.265575(7) 0.080446(7) 0.536306(7) 0.0188(4) Uani 1.000000 1 . . .
O4 O 0.393066(7) 0.221866(7) 0.437366(7) 0.0157(4) Uani 1.000000 1 . . .
O5 O 0.317286(7) 0.191312(7) 0.669236(7) 0.0189(4) Uani 1.000000 1 . . .
O6 O 0.0 0.235376(7) 0.75 0.0185(5) Uani 1.000000 2 S T P
O7 O 0.061493(7) 0.164105(7) 0.427857(7) 0.0193(4) Uani 1.000000 1 . . .
O8 O 0.164967(7) 0.077993(7) 0.303268(7) 0.0256(4) Uani 1.000000 1 . . .
O9 O 0.204242(7) 0.264732(7) 0.802126(7) 0.0238(4) Uani 1.000000 1 . . .
O10 O -0.043561(7) 0.125459(7) 0.614386(7) 0.0238(4) Uani 1.000000 1 . . .
O11 O 0.443515(7) 0.110304(7) 0.585261(7) 0.0277(5) Uani 1.000000 1 . . .
O12 O -0.066531(7) 0.244594(7) 0.499141(7) 0.0242(4) Uani 1.000000 1 . . .
O13 O 0.378398(7) 0.094723(7) 0.344713(7) 0.0300(5) Uani 1.000000 1 . . .
O14 O 0.098595(7) 0.038090(7) 0.523962(7) 0.0285(5) Uani 1.000000 1 . . .
O4W O 0.395118(7) 0.050128(7) 0.833192(7) 0.0363(5) Uani 1.000000 1 . . .
H4Wa H 0.446120(7) 0.058594(7) 0.866785(7) 0.0545(8) Uiso 1.000000 1 GR . .
H4Wb H 0.391211(7) 0.007157(7) 0.834861(7) 0.0545(8) Uiso 1.000000 1 GR . .
O3W O 0.392981(7) 0.120247(7) 1.075785(7) 0.0377(6) Uani 1.000000 1 . . .
H3Wa H 0.380318(7) 0.104045(7) 1.149003(7) 0.0565(8) Uiso 1.000000 1 GR . .
H3Wb H 0.389544(7) 0.162931(7) 1.085533(7) 0.0565(8) Uiso 1.000000 1 GR . .
O2W O 0.207478(7) 0.130022(7) 1.048911(7) 0.0460(6) Uani 1.000000 1 . . .
H2Wa H 0.213790(7) 0.172803(7) 1.052146(7) 0.0690(10) Uiso 1.000000 1 GR . .
H2Wb H 0.214650(7) 0.117086(7) 1.126928(7) 0.0690(10) Uiso 1.000000 1 GR . .
O1W O 0.212992(7) 0.062405(7) 0.808287(7) 0.0370(5) Uani 1.000000 1 . . .
H1Wa H 0.208338(7) 0.019475(7) 0.807938(7) 0.0555(8) Uiso 1.000000 1 GR . .
H1Wb H 0.231901(7) 0.072081(7) 0.734083(7) 0.0555(8) Uiso 1.000000 1 GR . .
O5W O 0.0 0.000181(7) 0.75 0.0426(7) Uani 1.000000 2 S T P
H5Wa H -0.0075921(4) 0.033477(7) 0.6986822(4) 0.0639(11) Uiso 0.500000 1 G . .
H5Wb H -0.0132946(4) 0.015662(7) 0.8235048(3) 0.0639(11) Uiso 0.500000 1 G . .
O6W O 0.0 0.265168(7) 0.25 0.0446(8) Uani 1.000000 2 S T P
H6Wa H -0.0468060(2) 0.258614(7) 0.2916751(5) 0.0670(12) Uiso 0.500000 1 G . .
H6Wb H 0.0305897(3) 0.229482(7) 0.2629389(6) 0.0670(12) Uiso 0.500000 1 G . .


loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 Mo3 3.2371(5) 7_556 ?
Mo1 Mo4 3.3833(6) . ?
Mo1 O1 1.9493(3) . ?
Mo1 O1 2.4923(4) 7_556 ?
Mo1 O2 1.8838(3) . ?
Mo1 O4 2.1492(3) 7_556 ?
Mo1 O5 1.7523(3) . ?
Mo1 O9 1.6956(3) . ?
Pd1 O4W 2.0450(3) . ?
Pd1 O3W 2.0424(3) . ?
Pd1 O2W 2.0395(3) . ?
Pd1 O1W 2.0289(3) . ?
Mo3 Mo5 3.2683(6) . ?
Mo3 O1 2.1893(3) 7_556 ?
Mo3 O3 1.9142(3) . ?
Mo3 O4 1.8988(4) . ?
Mo3 O5 2.3758(4) . ?
Mo3 O11 1.7364(3) . ?
Mo3 O13 1.7198(3) . ?
Mo4 Mo5 3.2622(4) . ?
Mo4 O2 2.2157(4) . ?
Mo4 O4 2.2285(3) 7_556 ?
Mo4 O6 1.9089(3) . ?
Mo4 O7 2.0046(3) . ?
Mo4 O10 1.7186(3) . ?
Mo4 O12 1.7133(2) . ?
Mo5 O1 2.2347(3) 7_556 ?
Mo5 O2 2.2966(4) . ?
Mo5 O3 1.9749(3) . ?
Mo5 O7 1.8757(3) . ?
Mo5 O8 1.7326(3) . ?
Mo5 O14 1.7132(3) . ?
O4W H4Wa 0.8700 . ?
O4W H4Wb 0.8702 . ?
O3W H3Wa 0.8701 . ?
O3W H3Wb 0.8700 . ?
O2W H2Wa 0.8700 . ?
O2W H2Wb 0.8700 . ?
O1W H1Wa 0.8700 . ?
O1W H1Wb 0.8700 . ?
O5W H5Wa 0.8700 . ?
O5W H5Wa 0.8700 2_556 ?
O5W H5Wb 0.8700 2_556 ?
O5W H5Wb 0.8700 . ?
H5Wa H5Wa 1.1040(2) 2_556 ?
H5Wa H5Wb 0.54220(6) 2_556 ?
O6W H6Wa 0.8701 2 ?
O6W H6Wa 0.8701 . ?
O6W H6Wb 0.8700 . ?
O6W H6Wb 0.8700 2 ?
H6Wa H6Wb 0.86802(11) 2 ?
H6Wb H6Wb 0.97470(17) 2 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Mo4 Mo1 Mo3 74.515(3) . 7_556 ?
O1 Mo1 Mo3 85.878(4) 7_556 7_556 ?
O1 Mo1 Mo3 41.271(4) . 7_556 ?
O1 Mo1 Mo4 112.523(5) . . ?
O1 Mo1 Mo4 82.948(4) 7_556 . ?
O2 Mo1 Mo3 110.817(5) . 7_556 ?
O2 Mo1 Mo4 37.698(5) . . ?
O2 Mo1 O1 141.279(6) . . ?
O2 Mo1 O1 76.124(5) . 7_556 ?
O4 Mo1 Mo3 34.315(4) 7_556 7_556 ?
O4 Mo1 Mo4 40.249(4) 7_556 . ?
O4 Mo1 O1 81.655(4) 7_556 7_556 ?
O4 Mo1 O1 73.363(6) 7_556 . ?
O4 Mo1 O2 76.787(6) 7_556 . ?
O5 Mo1 Mo3 138.263(6) . 7_556 ?
O5 Mo1 Mo4 137.869(7) . . ?
O5 Mo1 O1 76.206(5) . 7_556 ?
O5 Mo1 O1 97.301(7) . . ?
O5 Mo1 O2 101.105(8) . . ?
O5 Mo1 O4 157.554(5) . 7_556 ?
O9 Mo1 Mo3 93.412(6) . 7_556 ?
O9 Mo1 Mo4 97.185(5) . . ?
O9 Mo1 O1 103.600(8) . . ?
O9 Mo1 O1 179.218(8) . 7_556 ?
O9 Mo1 O2 104.452(7) . . ?
O9 Mo1 O4 97.943(7) . 7_556 ?
O9 Mo1 O5 104.150(6) . . ?
O3W Pd1 O4W 91.781(6) . . ?
O2W Pd1 O4W 178.576(6) . . ?
O2W Pd1 O3W 89.598(5) . . ?
O1W Pd1 O4W 87.884(5) . . ?
O1W Pd1 O3W 178.489(7) . . ?
O1W Pd1 O2W 90.728(5) . . ?
Mo5 Mo3 Mo1 77.095(3) . 7_556 ?
O1 Mo3 Mo1 35.965(4) 7_556 7_556 ?
O1 Mo3 Mo5 42.914(4) 7_556 . ?
O3 Mo3 Mo1 109.466(6) . 7_556 ?
O3 Mo3 Mo5 33.403(4) . . ?
O3 Mo3 O1 73.757(6) . 7_556 ?
O4 Mo3 Mo1 39.649(4) . 7_556 ?
O4 Mo3 Mo5 116.090(6) . . ?
O4 Mo3 O1 73.374(6) . 7_556 ?
O4 Mo3 O3 145.710(8) . . ?
O5 Mo3 Mo1 83.102(5) . 7_556 ?
O5 Mo3 Mo5 82.612(4) . . ?
O5 Mo3 O1 71.863(4) . 7_556 ?
O5 Mo3 O3 78.885(5) . . ?
O5 Mo3 O4 81.909(6) . . ?
O11 Mo3 Mo1 140.922(7) . 7_556 ?
O11 Mo3 Mo5 135.168(6) . . ?
O11 Mo3 O1 152.992(6) . 7_556 ?
O11 Mo3 O3 102.224(7) . . ?
O11 Mo3 O4 102.543(7) . . ?
O11 Mo3 O5 81.141(5) . . ?
O13 Mo3 Mo1 94.042(5) . 7_556 ?
O13 Mo3 Mo5 91.937(5) . . ?
O13 Mo3 O1 102.951(6) . 7_556 ?
O13 Mo3 O3 97.504(7) . . ?
O13 Mo3 O4 99.068(6) . . ?
O13 Mo3 O5 174.286(7) . . ?
O13 Mo3 O11 104.054(7) . . ?
Mo5 Mo4 Mo1 63.573(3) . . ?
O2 Mo4 Mo1 31.325(4) . . ?
O2 Mo4 Mo5 44.693(3) . . ?
O4 Mo4 Mo1 38.543(4) 7_556 . ?
O4 Mo4 Mo5 84.593(5) 7_556 . ?
O4 Mo4 O2 68.876(5) 7_556 . ?
O6 Mo4 Mo1 79.043(3) . . ?
O6 Mo4 Mo5 132.424(5) . . ?
O6 Mo4 O2 88.255(4) . . ?
O6 Mo4 O4 83.437(5) . 7_556 ?
O7 Mo4 Mo1 80.711(4) . . ?
O7 Mo4 Mo5 31.579(4) . . ?
O7 Mo4 O2 73.151(5) . . ?
O7 Mo4 O4 82.146(5) . 7_556 ?
O7 Mo4 O6 159.630(6) . . ?
O10 Mo4 Mo1 126.126(6) . . ?
O10 Mo4 Mo5 83.825(6) . . ?
O10 Mo4 O2 95.570(7) . . ?
O10 Mo4 O4 164.444(8) . 7_556 ?
O10 Mo4 O6 96.816(6) . . ?
O10 Mo4 O7 93.279(7) . . ?
O12 Mo4 Mo1 128.955(7) . . ?
O12 Mo4 Mo5 123.807(5) . . ?
O12 Mo4 O2 155.823(7) . . ?
O12 Mo4 O4 90.468(7) . 7_556 ?
O12 Mo4 O6 102.180(7) . . ?
O12 Mo4 O7 92.265(5) . . ?
O12 Mo4 O10 104.613(7) . . ?
Mo4 Mo5 Mo3 121.708(4) . . ?
O1 Mo5 Mo3 41.842(4) 7_556 . ?
O1 Mo5 Mo4 89.812(5) 7_556 . ?
O2 Mo5 Mo3 86.142(4) . . ?
O2 Mo5 Mo4 42.729(3) . . ?
O2 Mo5 O1 74.402(5) . 7_556 ?
O3 Mo5 Mo3 32.250(4) . . ?
O3 Mo5 Mo4 124.899(5) . . ?
O3 Mo5 O1 71.635(6) . 7_556 ?
O3 Mo5 O2 82.170(5) . . ?
O7 Mo5 Mo3 127.188(7) . . ?
O7 Mo5 Mo4 34.034(3) . . ?
O7 Mo5 O1 85.456(7) . 7_556 ?
O7 Mo5 O2 73.551(5) . . ?
O7 Mo5 O3 150.375(8) . . ?
O8 Mo5 Mo3 89.411(5) . . ?
O8 Mo5 Mo4 131.893(6) . . ?
O8 Mo5 O1 93.039(6) . 7_556 ?
O8 Mo5 O2 165.347(9) . . ?
O8 Mo5 O3 101.295(6) . . ?
O8 Mo5 O7 98.366(6) . . ?
O14 Mo5 Mo3 126.706(6) . . ?
O14 Mo5 Mo4 86.838(6) . . ?
O14 Mo5 O1 160.382(5) . 7_556 ?
O14 Mo5 O2 90.241(5) . . ?
O14 Mo5 O3 94.591(7) . . ?
O14 Mo5 O7 102.105(7) . . ?
O14 Mo5 O8 103.563(8) . . ?
Mo3 O1 Mo1 102.764(6) 7_556 . ?
Mo3 O1 Mo1 96.572(4) 7_556 7_556 ?
Mo5 O1 Mo1 95.456(5) 7_556 7_556 ?
Mo5 O1 Mo1 151.290(5) 7_556 . ?
Mo5 O1 Mo3 95.245(7) 7_556 7_556 ?
Mo4 O2 Mo1 110.977(8) . . ?
Mo5 O2 Mo1 113.433(6) . . ?
Mo5 O2 Mo4 92.578(5) . . ?
Mo5 O3 Mo3 114.348(7) . . ?
Mo3 O4 Mo1 106.036(6) . 7_556 ?
Mo4 O4 Mo1 101.208(6) 7_556 7_556 ?
Mo4 O4 Mo3 152.490(7) 7_556 . ?
Mo3 O5 Mo1 115.153(5) . . ?
Mo4 O6 Mo4 134.515(10) 2_556 . ?
Mo5 O7 Mo4 114.387(5) . . ?
H4Wa O4W Pd1 109.4 . . ?
H4Wb O4W Pd1 109.4 . . ?
H4Wb O4W H4Wa 104.5 . . ?
H3Wa O3W Pd1 109.4 . . ?
H3Wb O3W Pd1 109.4 . . ?
H3Wb O3W H3Wa 104.5 . . ?
H2Wa O2W Pd1 109.4 . . ?
H2Wb O2W Pd1 109.5 . . ?
H2Wb O2W H2Wa 104.5 . . ?
H1Wa O1W Pd1 109.4 . . ?
H1Wb O1W Pd1 109.4 . . ?
H1Wb O1W H1Wa 104.5 . . ?
H5Wa O5W H5Wa 78.7648(8) . 2_556 ?
H5Wb O5W H5Wa 104.5 . . ?
H5Wb O5W H5Wa 36.3 2_556 . ?
H5Wb O5W H5Wa 104.5 2_556 2_556 ?
H5Wb O5W H5Wa 36.3 . 2_556 ?
H5Wb O5W H5Wb 137.8803(8) . 2_556 ?
H5Wa H5Wa O5W 50.6176(4) 2_556 2_556 ?
H5Wb H5Wa O5W 71.8490(4) 2_556 2_556 ?
H5Wa H5Wb O5W 71.8390(4) 2_556 2_556 ?
H6Wa O6W H6Wa 162.4988(8) . 2 ?
H6Wb O6W H6Wa 104.5 . . ?
H6Wb O6W H6Wa 104.5 2 2 ?
H6Wb O6W H6Wa 59.8 . 2 ?
H6Wb O6W H6Wa 59.8 2 . ?
H6Wb O6W H6Wb 68.1324(8) 2 . ?
H6Wb H6Wa O6W 60.0744(4) 2 2 ?
H6Wa H6Wb O6W 60.0799(4) 2 . ?
H6Wb H6Wb O6W 55.9338(3) 2 . ?
H6Wb H6Wb H6Wa 96.4270(6) 2 2 ?

_olex2_submission_special_instructions 'No special instructions were received'
